#------------------------------------------------------------------------------
#$Date: 2019-11-26 09:46:18 +0200 (Tue, 26 Nov 2019) $
#$Revision: 243177 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/13/33/4133371.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4133371
loop_
_publ_author_name
'Xuan, Weimin'
'Pow, Robert'
'Watfa, Nancy'
'Zheng, Qi'
'Surman, Andrew J.'
'Long, De-Liang'
'Cronin, Leroy'
_publ_section_title
;
 Stereoselective Assembly of Gigantic Chiral Molybdenum Blue Wheels Using
 Lanthanide Ions and Amino Acids.
;
_journal_issue                   3
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              1242
_journal_page_last               1250
_journal_paper_doi               10.1021/jacs.8b09750
_journal_volume                  141
_journal_year                    2019
_chemical_absolute_configuration none
_chemical_formula_sum            'C86 H534 Ce4 Mo124 N16 Na2 O604'
_chemical_formula_weight         23962.28
_space_group_crystal_system      orthorhombic
_space_group_IT_number           18
_space_group_name_Hall           'P 2 2ab'
_space_group_name_H-M_alt        'P 21 21 2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2016/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   34.961(3)
_cell_length_b                   45.659(4)
_cell_length_c                   20.6838(14)
_cell_measurement_reflns_used    9125
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      26.3
_cell_measurement_theta_min      2.29
_cell_volume                     33017(5)
_computing_cell_refinement       Apex2
_computing_data_collection       Apex2
_computing_data_reduction        Apex2
_computing_molecular_graphics    Diamond3
_computing_publication_material  WinGX
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker Apex II Quasar'
_diffrn_measurement_method       'ω & φ scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1041
_diffrn_reflns_av_unetI/netI     0.0633
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       42
_diffrn_reflns_limit_h_min       -43
_diffrn_reflns_limit_k_max       56
_diffrn_reflns_limit_k_min       -56
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            399953
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.000
_diffrn_reflns_theta_min         0.984
_diffrn_source                   '1uS Microfocus x-ray'
_exptl_absorpt_coefficient_mu    2.653
_exptl_absorpt_correction_T_max  0.7454
_exptl_absorpt_correction_T_min  0.6453
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS-2014/5
_exptl_crystal_colour            'deep blue'
_exptl_crystal_density_diffrn    2.410
_exptl_crystal_density_method    none
_exptl_crystal_description       block
_exptl_crystal_F_000             22912
_exptl_crystal_size_max          0.500
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         1.680
_refine_diff_density_min         -1.309
_refine_diff_density_rms         0.215
_refine_ls_abs_structure_details
;
 Flack x determined using 23434 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   -0.034(6)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.083
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     3372
_refine_ls_number_reflns         64861
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.083
_refine_ls_R_factor_all          0.0608
_refine_ls_R_factor_gt           0.0476
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0612P)²+205.2108P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1212
_refine_ls_wR_factor_ref         0.1345
_reflns_Friedel_coverage         0.888
_reflns_Friedel_fraction_full    0.999
_reflns_Friedel_fraction_max     0.999
_reflns_number_gt                56409
_reflns_number_total             64861
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            4-l-wx924.cif
_cod_data_source_block           wx924
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_atom_sites_solution_primary' value 'direct methods' was
changed to 'direct'.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        33017(4)
_cod_database_code               4133371
_shelx_shelxl_version_number     2016/6
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.351
_shelx_estimated_absorpt_t_max   0.777
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.63896(4) 0.10857(3) 0.67403(6) 0.0225(3) Uani 1 1 d . . . . .
Mo2 Mo 0.70052(4) 0.17522(3) 0.67031(6) 0.0219(3) Uani 1 1 d . . . . .
Mo3 Mo 0.69732(4) 0.18182(3) 0.82983(6) 0.0225(3) Uani 1 1 d . . . . .
Mo4 Mo 0.77788(4) 0.23390(3) 0.83247(6) 0.0225(3) Uani 1 1 d . . . . .
Mo5 Mo 0.77173(4) 0.23492(3) 0.67132(6) 0.0211(2) Uani 1 1 d . . . . .
Mo6 Mo 0.86742(4) 0.27907(3) 0.66772(6) 0.0231(3) Uani 1 1 d . . . . .
Mo7 Mo 0.86993(4) 0.27633(3) 0.82861(6) 0.0244(3) Uani 1 1 d . . . . .
Mo8 Mo 0.96848(4) 0.30074(3) 0.65293(6) 0.0246(3) Uani 1 1 d . . . . .
Mo9 Mo 0.82060(4) -0.29915(3) 0.64952(6) 0.0230(3) Uani 1 1 d . . . . .
Mo10 Mo 0.79902(4) -0.23580(3) 0.73944(6) 0.0244(3) Uani 1 1 d . . . . .
Mo11 Mo 0.81860(4) -0.30174(3) 0.81080(6) 0.0225(3) Uani 1 1 d . . . . .
Mo12 Mo 0.64935(4) -0.20768(3) 0.83623(6) 0.0223(3) Uani 1 1 d . . . . .
Mo13 Mo 0.60044(4) -0.12800(3) 0.84588(6) 0.0233(3) Uani 1 1 d . . . . .
Mo14 Mo 0.59964(4) -0.12876(3) 0.68540(6) 0.0238(3) Uani 1 1 d . . . . .
Mo15 Mo 0.59124(4) -0.04774(3) 0.84898(6) 0.0244(3) Uani 1 1 d . . . . .
Mo18 Mo 0.59585(4) 0.03526(3) 0.68394(6) 0.0232(3) Uani 1 1 d . . . . .
Mo19 Mo 0.96721(4) 0.30708(3) 0.81415(6) 0.0255(3) Uani 1 1 d . . . . .
Mo20 Mo 0.71863(4) -0.25934(3) 0.66129(6) 0.0222(3) Uani 1 1 d . . . . .
Mo21 Mo 0.94213(4) 0.23082(3) 0.57891(6) 0.0230(3) Uani 1 1 d . . . . .
Mo22 Mo 1.07808(4) 0.31628(3) 0.80827(6) 0.0245(3) Uani 1 1 d . . . . .
Mo23 Mo 0.72433(4) -0.26408(3) 0.82115(6) 0.0215(3) Uani 1 1 d . . . . .
Mo24 Mo 0.68275(4) -0.14273(3) 0.76028(6) 0.0257(3) Uani 1 1 d . . . . .
Mo25 Mo 0.79353(4) -0.23905(3) 0.57598(6) 0.0232(3) Uani 1 1 d . . . . .
Mo26 Mo 1.12139(4) 0.25011(3) 0.90133(6) 0.0245(3) Uani 1 1 d . . . . .
Mo27 Mo 0.84840(4) 0.21873(3) 0.58984(6) 0.0254(3) Uani 1 1 d . . . . .
Mo28 Mo 0.79244(4) 0.15983(3) 0.59178(6) 0.0239(3) Uani 1 1 d . . . . .
Mo29 Mo 0.64631(4) -0.20154(3) 0.67552(6) 0.0228(3) Uani 1 1 d . . . . .
Mo30 Mo 0.74789(4) -0.20005(3) 0.92087(6) 0.0241(3) Uani 1 1 d . . . . .
Mo31 Mo 0.58146(4) -0.04946(3) 0.68709(6) 0.0246(3) Uani 1 1 d . . . . .
Mo32 Mo 0.85834(4) 0.21298(3) 0.75304(6) 0.0319(3) Uani 1 1 d . . . . .
Mo33 Mo 1.02957(4) 0.26969(3) 0.89766(6) 0.0248(3) Uani 1 1 d . . . . .
Mo34 Mo 0.66140(4) -0.01174(3) 0.76281(6) 0.0276(3) Uani 1 1 d . . . . .
Mo35 Mo 0.78064(4) 0.08971(3) 0.99848(7) 0.0312(3) Uani 1 1 d . . . . .
Mo36 Mo 1.03057(4) 0.25664(3) 0.73420(6) 0.0275(3) Uani 1 1 d . . . . .
Mo37 Mo 0.69293(4) 0.05243(3) 0.92869(6) 0.0276(3) Uani 1 1 d . . . . .
Mo38 Mo 0.71379(4) 0.12329(3) 0.91434(6) 0.0247(3) Uani 1 1 d . . . . .
Mo39 Mo 0.79280(4) 0.16468(3) 0.91697(6) 0.0257(3) Uani 1 1 d . . . . .
Mo40 Mo 0.94693(4) 0.23388(3) 0.90441(6) 0.0269(3) Uani 1 1 d . . . . .
Mo41 Mo 0.63445(4) 0.11051(3) 0.83592(6) 0.0230(3) Uani 1 1 d . . . . .
Mo42 Mo 1.07463(4) 0.30813(3) 0.64681(6) 0.0238(3) Uani 1 1 d . . . . .
Mo43 Mo 0.67649(4) -0.15147(3) 0.92268(6) 0.0248(3) Uani 1 1 d . . . . .
Mo44 Mo 0.60407(4) 0.03315(3) 0.84487(6) 0.0238(3) Uani 1 1 d . . . . .
Mo45 Mo 0.64260(4) -0.01290(3) 0.59896(6) 0.0251(3) Uani 1 1 d . . . . .
Mo46 Mo 0.67381(4) -0.07899(3) 0.93564(6) 0.0273(3) Uani 1 1 d . . . . .
Mo47 Mo 0.69011(4) 0.04973(3) 0.58823(7) 0.0302(3) Uani 1 1 d . . . . .
Mo48 Mo 0.97726(4) 0.19267(3) 0.42292(6) 0.0299(3) Uani 1 1 d . . . . .
Mo49 Mo 0.82114(5) 0.10927(3) 0.44929(7) 0.0354(3) Uani 1 1 d . . . . .
Mo50 Mo 0.73378(5) -0.18215(3) 0.58823(9) 0.0252(3) Uani 0.9 1 d . . P A 1
Mo51 Mo 0.72521(4) 0.11608(3) 0.75227(6) 0.0292(3) Uani 1 1 d . . . . .
Mo52 Mo 0.66628(4) -0.08360(3) 0.59172(7) 0.0305(3) Uani 1 1 d . . . . .
Mo53 Mo 0.88718(4) 0.16648(3) 0.50100(8) 0.0384(4) Uani 1 1 d . . . . .
Mo54 Mo 0.74349(5) 0.02269(3) 1.08062(6) 0.0331(3) Uani 1 1 d . . . . .
Mo55 Mo 1.07831(4) 0.19220(4) 0.42651(7) 0.0411(4) Uani 1 1 d . . . . .
Mo56 Mo 0.73923(5) -0.05458(3) 1.07547(7) 0.0390(4) Uani 1 1 d . . . . .
Mo57 Mo 1.04236(4) 0.20862(4) 0.98479(7) 0.0353(3) Uani 1 1 d . . . . .
Mo58 Mo 0.86358(7) 0.13654(5) 1.04760(11) 0.0281(5) Uani 0.86 1 d . . P B 1
Mo59 Mo 0.95392(4) 0.16362(3) 1.00171(8) 0.0365(3) Uani 1 1 d . . . . .
Mo60 Mo 0.88792(9) -0.24277(7) 0.56486(13) 0.0301(6) Uani 0.85 1 d . . P C 1
Mo61 Mo 0.77328(6) 0.04365(3) 0.47180(9) 0.0508(5) Uani 1 1 d . . . . .
Mo62 Mo 0.82784(5) -0.17995(4) 0.50007(10) 0.0538(5) Uani 1 1 d . . . . .
Mo63 Mo 0.74785(9) -0.13043(6) 1.01883(13) 0.0330(6) Uani 0.78 1 d . . P D 1
Mo64 Mo 0.72175(6) -0.02317(3) 0.51174(10) 0.0550(5) Uani 1 1 d . . . . .
M50 Mo 0.7264(6) -0.1880(5) 0.5651(10) 0.042(6) Uiso 0.1 1 d . . P E 2
M58 Mo 0.8675(4) 0.1269(3) 1.0278(7) 0.025(3) Uani 0.14 1 d . . P F 2
M60 Mo 1.1151(5) 0.2503(4) 0.5427(8) 0.032(4) Uani 0.15 1 d . . P G 2
M63 Mo 0.7549(3) -0.12463(19) 0.9943(4) 0.0255(17) Uani 0.24 1 d . . P H 2
Ce1 Ce 0.84371(3) -0.18634(2) 1.03233(4) 0.02661(18) Uani 1 1 d . . . . .
Ce2 Ce 0.75181(3) -0.11016(2) 0.46843(4) 0.0338(2) Uani 1 1 d . . . . .
Na1 Na 0.7929(14) -0.1910(11) 1.249(2) 0.091(13) Uiso 0.25 1 d . . P . .
Na2 Na 0.9176(10) 0.3165(7) 0.4924(15) 0.096(9) Uiso 0.4 1 d . . P . .
O1 O 0.7321(5) 0.0516(5) 0.3915(8) 0.083(6) Uani 1 1 d . . . . .
O2 O 0.8065(5) 0.0330(3) 0.4155(10) 0.084(6) Uani 1 1 d . . . . .
O3 O 0.7787(4) 0.0850(2) 0.4633(5) 0.036(3) Uani 1 1 d . . . . .
O4 O 0.7228(4) 0.0572(3) 0.5256(6) 0.047(3) Uani 1 1 d . . . . .
O5 O 0.6449(4) 0.0574(3) 0.5065(5) 0.048(3) Uani 1 1 d . . . . .
O6 O 0.7187(3) 0.0414(2) 0.6529(6) 0.036(3) Uani 1 1 d . . . . .
O7 O 0.6703(3) 0.0857(2) 0.6143(5) 0.028(2) Uani 1 1 d . . . . .
O8 O 0.6402(3) 0.0292(2) 0.6264(5) 0.027(2) Uani 1 1 d . . . . .
O9 O 0.5577(3) 0.0346(2) 0.6350(5) 0.029(2) Uani 1 1 d . . . . .
O10 O 0.6083(3) 0.0748(2) 0.6844(5) 0.025(2) Uani 1 1 d . . . . .
O11 O 0.5750(3) 0.0323(2) 0.7656(5) 0.025(2) Uani 1 1 d . . . . .
O12 O 0.5679(3) 0.0298(2) 0.8976(5) 0.032(2) Uani 1 1 d . . . . .
O13 O 0.6104(3) 0.0750(2) 0.8350(5) 0.024(2) Uani 1 1 d . . . . .
O14 O 0.6193(3) 0.1238(2) 0.7550(5) 0.024(2) Uani 1 1 d . . . . .
O15 O 0.6484(3) 0.0346(2) 0.9040(5) 0.031(2) Uani 1 1 d . . . . .
O16 O 0.6087(3) 0.1306(2) 0.8869(5) 0.031(2) Uani 1 1 d . . . . .
O17 O 0.6132(3) 0.1293(2) 0.6234(5) 0.033(3) Uani 1 1 d . . . . .
O18 O 0.6784(3) 0.0894(2) 0.7553(5) 0.023(2) Uani 1 1 d . . . . .
O19 O 0.6854(3) 0.1334(2) 0.6857(4) 0.026(2) Uani 1 1 d . . . . .
O20 O 0.6754(3) 0.0928(2) 0.8909(5) 0.025(2) Uani 1 1 d . . . . .
O21 O 0.7210(4) 0.0447(3) 0.8645(6) 0.040(3) Uani 1 1 d . . . . .
O22 O 0.7110(4) 0.0308(3) 0.9922(6) 0.041(3) Uani 1 1 d . . . . .
O23 O 0.6521(4) 0.0700(3) 1.0096(6) 0.047(3) Uani 1 1 d . . . . .
O24 O 0.6864(3) 0.1396(2) 0.9714(5) 0.031(2) Uani 1 1 d . . . . .
O25 O 0.7264(3) 0.0868(2) 0.9616(5) 0.030(2) Uani 1 1 d . . . . .
O26 O 0.6820(3) 0.1381(2) 0.8354(4) 0.023(2) Uani 1 1 d . . . . .
O27 O 0.6639(3) 0.1943(2) 0.8818(5) 0.029(2) Uani 1 1 d . . . . .
O28 O 0.7359(3) 0.1620(2) 0.8866(5) 0.024(2) Uani 1 1 d . . . . .
O29 O 0.7436(3) 0.1060(2) 0.8286(5) 0.025(2) Uani 1 1 d . . . . .
O30 O 0.7378(3) 0.1568(2) 0.7516(5) 0.023(2) Uani 1 1 d . . . . .
O31 O 0.7545(3) 0.0995(3) 0.7001(5) 0.035(3) Uani 1 1 d . . . . .
O32 O 0.6741(3) 0.1867(2) 0.7498(5) 0.023(2) Uani 1 1 d . . . . .
O33 O 0.6666(3) 0.1834(2) 0.6159(5) 0.031(2) Uani 1 1 d . . . . .
O34 O 0.7415(3) 0.1596(2) 0.6157(5) 0.025(2) Uani 1 1 d . . . . .
O35 O 0.7298(3) 0.2108(2) 0.6757(5) 0.026(2) Uani 1 1 d . . . . .
O36 O 0.7311(3) 0.2130(2) 0.8250(5) 0.027(2) Uani 1 1 d . . . . .
O37 O 0.7666(3) 0.1272(2) 0.9500(5) 0.028(2) Uani 1 1 d . . . . .
O38 O 0.7438(4) 0.1188(3) 1.0763(6) 0.045(3) Uani 1 1 d . . . . .
O39 O 0.7683(4) 0.0605(2) 1.0523(6) 0.038(3) Uani 1 1 d . . . . .
O40 O 0.8037(4) 0.0732(3) 0.9370(6) 0.042(3) Uani 1 1 d . . . . .
O41 O 0.8184(4) 0.1086(3) 1.0387(6) 0.038(3) Uani 1 1 d . . . B 1
O42 O 0.8280(3) 0.1608(3) 0.9765(6) 0.037(3) Uani 1 1 d . . . B 1
O43 O 0.8119(3) 0.1488(2) 0.8493(5) 0.031(2) Uani 1 1 d . . . . .
O44 O 0.7590(3) 0.1810(3) 1.0089(5) 0.034(3) Uani 1 1 d . . . . .
O45 O 0.7941(3) 0.2036(2) 0.8947(5) 0.028(2) Uani 1 1 d . . . . .
O46 O 0.8760(4) 0.1174(3) 0.9528(6) 0.055(4) Uani 1 1 d . . . B 1
O47 O 0.8908(4) 0.1117(3) 1.0888(6) 0.048(3) Uani 1 1 d . . . B 1
O48 O 0.8414(4) 0.1563(3) 1.1074(6) 0.048(3) Uani 1 1 d . . . B 1
O49 O 0.9005(3) 0.1626(3) 1.0234(6) 0.036(3) Uani 1 1 d . . . B 1
O50 O 0.8012(3) 0.2033(2) 0.7547(5) 0.029(2) Uani 1 1 d . . . . .
O51 O 0.7671(3) 0.2535(2) 0.7511(5) 0.023(2) Uani 1 1 d . . . . .
O52 O 0.7668(3) 0.2622(2) 0.8813(5) 0.029(2) Uani 1 1 d . . . . .
O53 O 0.7966(3) 0.2043(2) 0.6169(4) 0.023(2) Uani 1 1 d . . . . .
O54 O 0.7578(3) 0.2605(2) 0.6184(5) 0.028(2) Uani 1 1 d . . . . .
O55 O 0.8139(3) 0.1474(3) 0.6596(5) 0.035(3) Uani 1 1 d . . . . .
O56 O 0.7636(3) 0.1820(2) 0.5015(5) 0.032(3) Uani 1 1 d . . . . .
O57 O 0.7986(3) 0.1312(2) 0.5349(5) 0.033(3) Uani 1 1 d . . . . .
O58 O 0.7818(4) 0.1403(3) 0.4046(6) 0.052(4) Uani 1 1 d . . . . .
O59 O 0.8544(5) 0.0897(3) 0.5013(9) 0.075(5) Uani 1 1 d . . . . .
O60 O 0.8373(4) 0.0979(3) 0.3770(7) 0.060(4) Uani 1 1 d . . . . .
O61 O 0.8331(3) 0.2428(2) 0.8181(5) 0.029(2) Uani 1 1 d . . . . .
O62 O 0.8450(3) 0.2968(2) 0.8817(5) 0.032(2) Uani 1 1 d . . . . .
O63 O 0.9154(3) 0.2986(2) 0.8155(5) 0.028(2) Uani 1 1 d . . . . .
O64 O 0.8999(3) 0.2504(2) 0.8836(5) 0.030(2) Uani 1 1 d . . . . .
O65 O 0.8503(3) 0.2922(2) 0.7482(5) 0.026(2) Uani 1 1 d . . . . .
O66 O 0.8919(3) 0.2455(2) 0.7472(5) 0.029(2) Uani 1 1 d . . . . .
O67 O 0.8774(4) 0.1896(2) 0.8068(5) 0.035(3) Uani 1 1 d . . . . .
O68 O 0.8293(3) 0.2441(2) 0.6671(5) 0.022(2) Uani 1 1 d . . . . .
O69 O 0.8682(3) 0.1958(2) 0.6763(5) 0.027(2) Uani 1 1 d . . . . .
O70 O 0.8896(3) 0.2472(2) 0.6133(5) 0.025(2) Uani 1 1 d . . . . .
O71 O 0.8419(3) 0.2997(2) 0.6164(5) 0.030(2) Uani 1 1 d . . . . .
O72 O 0.8306(3) 0.2402(2) 0.5303(5) 0.027(2) Uani 1 1 d . . . . .
O73 O 0.8395(3) 0.1796(2) 0.5508(5) 0.029(2) Uani 1 1 d . . . . .
O74 O 0.9033(4) 0.1423(3) 0.5548(8) 0.055(4) Uani 1 1 d . . . . .
O75 O 0.8971(3) 0.2046(2) 0.5508(4) 0.023(2) Uani 1 1 d . . . . .
O76 O 0.8562(4) 0.1450(3) 0.4505(8) 0.064(5) Uani 1 1 d . . . . .
O77 O 0.8674(4) 0.2039(3) 0.4292(6) 0.052(4) Uani 1 1 d . . . . .
O78 O 0.9291(4) 0.1721(3) 0.4536(6) 0.046(3) Uani 1 1 d . . . . .
O79 O 0.9158(3) 0.2561(3) 0.4891(5) 0.035(3) Uani 1 1 d . . . . .
O80 O 0.9532(3) 0.2118(3) 0.6467(5) 0.032(3) Uani 1 1 d . . . . .
O81 O 0.9512(4) 0.1494(3) 0.9265(7) 0.058(4) Uani 1 1 d . . . . .
O82 O 0.9683(4) 0.1347(3) 1.0469(7) 0.054(4) Uani 1 1 d . . . . .
O83 O 0.9517(4) 0.1939(3) 1.0903(7) 0.053(4) Uani 1 1 d . . . . .
O84 O 0.9378(3) 0.2069(3) 0.9611(6) 0.039(3) Uani 1 1 d . . . . .
O85 O 1.0052(3) 0.1810(3) 0.9954(6) 0.043(3) Uani 1 1 d . . . . .
O86 O 0.9348(3) 0.2646(3) 0.9927(5) 0.039(3) Uani 1 1 d . . . . .
O87 O 0.9566(3) 0.2152(3) 0.8358(5) 0.037(3) Uani 1 1 d . . . . .
O88 O 1.0014(3) 0.2364(3) 0.9377(5) 0.031(2) Uani 1 1 d . . . . .
O89 O 0.9740(3) 0.2727(2) 0.8719(5) 0.027(2) Uani 1 1 d . . . . .
O90 O 0.9715(4) 0.3367(3) 0.8618(5) 0.038(3) Uani 1 1 d . . . . .
O91 O 0.9750(3) 0.2668(2) 0.7372(5) 0.025(2) Uani 1 1 d . . . . .
O92 O 0.9710(3) 0.3236(2) 0.7322(5) 0.031(2) Uani 1 1 d . . . . .
O93 O 0.9652(3) 0.2661(2) 0.5968(5) 0.026(2) Uani 1 1 d . . . . .
O94 O 0.9145(3) 0.2967(2) 0.6654(5) 0.028(2) Uani 1 1 d . . . . .
O95 O 0.9722(4) 0.3279(2) 0.5995(5) 0.036(3) Uani 1 1 d . . . . .
O96 O 0.9704(3) 0.2140(2) 0.5180(5) 0.028(2) Uani 1 1 d . . . . .
O97 O 0.9975(4) 0.1603(3) 0.4959(6) 0.042(3) Uani 1 1 d . . . . .
O98 O 0.9834(4) 0.1683(3) 0.3622(6) 0.050(3) Uani 1 1 d . . . . .
O99 O 0.9549(4) 0.2217(3) 0.3874(7) 0.055(4) Uani 1 1 d . . . . .
O100 O 1.0270(3) 0.2081(3) 0.4300(5) 0.036(3) Uani 1 1 d . . . . .
O101 O 1.0247(3) 0.2966(2) 0.8149(5) 0.025(2) Uani 1 1 d . . . . .
O102 O 1.0328(3) 0.2405(2) 0.8123(4) 0.025(2) Uani 1 1 d . . . . .
O103 O 1.0258(3) 0.2957(2) 0.9548(5) 0.030(2) Uani 1 1 d . . . . .
O104 O 1.0374(4) 0.2272(3) 1.0593(6) 0.049(3) Uani 1 1 d . . . . .
O105 O 1.0848(3) 0.1905(3) 0.9958(6) 0.035(3) Uani 1 1 d . . . . .
O106 O 1.0677(3) 0.2437(2) 0.9403(5) 0.028(2) Uani 1 1 d . . . . .
O107 O 1.0436(4) 0.1907(3) 0.8839(6) 0.042(3) Uani 1 1 d . . . . .
O108 O 1.0818(3) 0.2829(2) 0.8693(5) 0.025(2) Uani 1 1 d . . . . .
O109 O 1.0671(3) 0.3445(2) 0.8556(5) 0.032(3) Uani 1 1 d . . . . .
O110 O 0.8690(3) -0.3171(2) 0.8046(5) 0.025(2) Uani 1 1 d . . . . .
O111 O 1.0798(3) 0.2748(2) 0.7324(5) 0.026(2) Uani 1 1 d . . . . .
O112 O 1.0696(3) 0.3307(2) 0.7258(5) 0.028(2) Uani 1 1 d . . . . .
O113 O 1.0332(3) 0.2282(2) 0.6837(5) 0.030(2) Uani 1 1 d . . . . .
O114 O 1.0234(3) 0.2898(2) 0.6658(5) 0.025(2) Uani 1 1 d . . . . .
O115 O 1.0605(3) 0.3339(3) 0.5933(5) 0.036(3) Uani 1 1 d . . . . .
O116 O 0.9168(3) -0.2742(2) 0.5905(5) 0.030(2) Uani 1 1 d . . . C 1
O117 O 0.8925(4) -0.2214(3) 0.6312(7) 0.046(3) Uani 1 1 d . . . C 1
O118 O 1.0863(4) 0.2248(4) 0.5047(7) 0.059(4) Uani 1 1 d . . . . .
O119 O 1.0601(4) 0.1695(4) 0.5157(6) 0.070(5) Uani 1 1 d . . . . .
O120 O 1.0685(4) 0.1618(3) 0.3806(6) 0.049(3) Uani 1 1 d . . . . .
O121 O 1.0964(5) 0.2161(4) 0.3725(8) 0.070(5) Uani 1 1 d . . . . .
O122 O 0.8731(4) -0.1775(4) 0.4619(8) 0.071(5) Uani 1 1 d . . . . .
O123 O 0.8720(4) -0.2745(4) 0.4825(5) 0.054(4) Uani 1 1 d . . . C 1
O124 O 0.8379(3) -0.2646(2) 0.5991(5) 0.026(2) Uani 1 1 d . . . C 1
O125 O 0.8712(3) -0.3124(2) 0.6497(5) 0.026(2) Uani 1 1 d . . . . .
O126 O 1.1140(3) 0.2275(2) 0.8371(5) 0.032(2) Uani 1 1 d . . . . .
O127 O 1.1245(3) 0.2848(3) 0.9853(5) 0.037(3) Uani 1 1 d . . . . .
O128 O 1.1429(3) 0.2279(2) 0.9608(5) 0.032(2) Uani 1 1 d . . . . .
O129 O 0.8400(3) -0.2738(2) 0.8725(5) 0.026(2) Uani 1 1 d . . . . .
O130 O 0.7955(3) -0.3253(2) 0.8589(5) 0.035(3) Uani 1 1 d . . . . .
O131 O 0.8057(3) -0.3170(2) 0.7273(5) 0.026(2) Uani 1 1 d . . . . .
O132 O 0.8397(3) -0.2668(2) 0.7344(4) 0.023(2) Uani 1 1 d . . . . .
O133 O 0.8000(3) -0.3205(2) 0.5944(5) 0.033(3) Uani 1 1 d . . . . .
O134 O 0.8393(3) -0.2231(3) 0.5314(5) 0.031(2) Uani 1 1 d . . . C 1
O135 O 0.8055(4) -0.1997(3) 0.4179(6) 0.051(4) Uani 1 1 d . . . . .
O136 O 0.8044(4) -0.1476(3) 0.4826(6) 0.043(3) Uani 1 1 d . . . . .
O137 O 0.7815(3) -0.1986(2) 0.5430(5) 0.030(2) Uani 1 1 d . . . A 1
O138 O 0.7764(3) -0.2606(2) 0.5162(5) 0.028(2) Uani 1 1 d . . . . .
O139 O 0.8462(5) -0.1669(3) 0.5838(7) 0.063(4) Uani 1 1 d . . . . .
O140 O 0.8107(3) -0.2175(2) 0.6660(5) 0.026(2) Uani 1 1 d . . . . .
O141 O 0.8899(5) -0.1941(5) 1.1252(7) 0.086(6) Uani 1 1 d . . . . .
O142 O 0.8239(5) -0.2318(3) 1.0912(6) 0.055(4) Uani 1 1 d . . . . .
O143 O 0.8739(4) -0.1368(3) 1.0417(9) 0.067(5) Uani 1 1 d . . . . .
O144 O 0.8431(4) -0.1655(3) 0.9177(6) 0.053(4) Uani 1 1 d . . . . .
O145 O 0.7920(4) -0.1471(3) 1.0263(6) 0.044(3) Uani 1 1 d . . . D 1
O146 O 0.7832(3) -0.2033(2) 0.9800(5) 0.029(2) Uani 1 1 d . . . . .
O147 O 0.7088(3) -0.2215(3) 0.9988(5) 0.038(3) Uani 1 1 d . . . . .
O148 O 0.7693(4) -0.1801(2) 0.8614(5) 0.035(3) Uani 1 1 d . . . . .
O149 O 0.7457(3) -0.2365(2) 0.8845(5) 0.027(2) Uani 1 1 d . . . . .
O150 O 0.7155(3) -0.2932(2) 0.8674(5) 0.030(2) Uani 1 1 d . . . . .
O151 O 0.8158(3) -0.2133(2) 0.7969(5) 0.026(2) Uani 1 1 d . . . . .
O152 O 0.7791(3) -0.2711(2) 0.7974(5) 0.025(2) Uani 1 1 d . . . . .
O153 O 0.7449(3) -0.2305(2) 0.7418(5) 0.025(2) Uani 1 1 d . . . . .
O154 O 0.7115(3) -0.2808(2) 0.7384(4) 0.023(2) Uani 1 1 d . . . . .
O155 O 0.7776(3) -0.2675(2) 0.6533(4) 0.024(2) Uani 1 1 d . . . . .
O156 O 0.7408(3) -0.2279(2) 0.6078(4) 0.023(2) Uani 1 1 d . . . A 1
O157 O 0.7066(3) -0.2850(2) 0.6066(5) 0.029(2) Uani 1 1 d . . . . .
O158 O 0.8145(6) -0.0847(4) 0.4666(13) 0.106(8) Uani 1 1 d . . . . .
O159 O 0.7714(5) -0.1010(4) 0.5861(6) 0.062(4) Uani 1 1 d . . . . .
O160 O 0.7333(4) -0.1519(2) 0.5383(6) 0.045(3) Uani 1 1 d . . . A 1
O161 O 0.7077(4) -0.2039(3) 0.4936(5) 0.041(3) Uani 1 1 d . . . A 1
O162 O 0.7565(4) -0.1714(3) 0.6551(6) 0.041(3) Uani 1 1 d . . . A 1
O163 O 0.6740(3) -0.2375(2) 0.6705(5) 0.025(2) Uani 1 1 d . . . . .
O164 O 0.6838(3) -0.1856(2) 0.6154(5) 0.030(2) Uani 1 1 d . . . A 1
O165 O 0.6087(3) -0.2077(2) 0.6275(5) 0.032(3) Uani 1 1 d . . . . .
O166 O 0.6905(3) -0.1871(2) 0.7553(5) 0.024(2) Uani 1 1 d . . . . .
O167 O 0.6912(3) -0.1911(2) 0.8905(5) 0.025(2) Uani 1 1 d . . . . .
O168 O 0.7265(3) -0.1629(2) 0.9627(5) 0.029(2) Uani 1 1 d . . . D 1
O169 O 0.7734(4) -0.1167(4) 0.9185(7) 0.060(4) Uani 1 1 d . . . D 1
O170 O 0.7233(5) -0.1412(3) 1.0887(6) 0.055(4) Uani 1 1 d . . . D 1
O171 O 0.7575(4) -0.0921(3) 1.0373(7) 0.053(4) Uani 1 1 d . . . D 1
O172 O 0.6976(3) -0.1175(2) 0.9685(5) 0.027(2) Uani 1 1 d . . . D 1
O173 O 0.6458(3) -0.1640(2) 0.9792(5) 0.031(2) Uani 1 1 d . . . . .
O174 O 0.6454(3) -0.1162(2) 0.8987(5) 0.028(2) Uani 1 1 d . . . . .
O175 O 0.7075(3) -0.1381(2) 0.8339(5) 0.024(2) Uani 1 1 d . . . . .
O176 O 0.6405(3) -0.1625(2) 0.8437(4) 0.023(2) Uani 1 1 d . . . . .
O177 O 0.6156(3) -0.2178(2) 0.8892(5) 0.027(2) Uani 1 1 d . . . . .
O178 O 0.6235(3) -0.2112(2) 0.7572(5) 0.025(2) Uani 1 1 d . . . . .
O179 O 0.7141(3) -0.1299(2) 0.7059(5) 0.027(2) Uani 1 1 d . . . . .
O181 O 0.7800(5) -0.0483(3) 1.1193(7) 0.060(4) Uani 1 1 d . . . . .
O182 O 0.7092(5) -0.0685(3) 1.1297(7) 0.065(4) Uani 1 1 d . . . . .
O183 O 0.7673(4) -0.0407(3) 0.9832(6) 0.046(3) Uani 1 1 d . . . . .
O184 O 0.7796(4) 0.0150(3) 1.1338(6) 0.047(3) Uani 1 1 d . . . . .
O185 O 0.7208(4) -0.0150(3) 1.0742(5) 0.038(3) Uani 1 1 d . . . . .
O186 O 0.7094(5) 0.0392(3) 1.1265(8) 0.060(4) Uani 1 1 d . . . . .
O187 O 0.7809(4) 0.0069(3) 0.9986(6) 0.042(3) Uani 1 1 d . . . . .
O188 O 0.6955(4) -0.0595(2) 0.9999(5) 0.035(3) Uani 1 1 d . . . . .
O189 O 0.6290(4) -0.0910(3) 1.0161(6) 0.042(3) Uani 1 1 d . . . . .
O190 O 0.6342(3) -0.0557(2) 0.9083(5) 0.031(2) Uani 1 1 d . . . . .
O191 O 0.6990(3) -0.0148(3) 0.8118(5) 0.036(3) Uani 1 1 d . . . . .
O192 O 0.7049(4) -0.0747(3) 0.8726(6) 0.038(3) Uani 1 1 d . . . . .
O193 O 0.6395(3) -0.1596(2) 0.6994(5) 0.028(2) Uani 1 1 d . . . . .
O194 O 0.6443(3) -0.1141(2) 0.7645(5) 0.025(2) Uani 1 1 d . . . . .
O195 O 0.6976(4) -0.0790(2) 0.6534(6) 0.038(3) Uani 1 1 d . . . . .
O196 O 0.7501(5) -0.0222(4) 0.5914(9) 0.075(5) Uani 1 1 d . . . . .
O197 O 0.6928(4) -0.1001(3) 0.5295(6) 0.044(3) Uani 1 1 d . . . . .
O198 O 0.7402(4) -0.0556(3) 0.4848(7) 0.054(4) Uani 1 1 d . . . . .
O199 O 0.7464(6) 0.0061(3) 0.4753(10) 0.104(8) Uani 1 1 d . . . . .
O200 O 0.6855(7) -0.0210(4) 0.4315(6) 0.083(6) Uani 1 1 d . . . . .
O201 O 0.5713(3) -0.1433(2) 0.9006(5) 0.032(2) Uani 1 1 d . . . . .
O202 O 0.5577(3) -0.0376(2) 0.9022(5) 0.033(3) Uani 1 1 d . . . . .
O203 O 0.5782(3) -0.1393(2) 0.7673(5) 0.027(2) Uani 1 1 d . . . . .
O204 O 0.5847(3) -0.0891(2) 0.8443(5) 0.028(2) Uani 1 1 d . . . . .
O205 O 0.6171(3) -0.0093(2) 0.8317(5) 0.026(2) Uani 1 1 d . . . . .
O206 O 0.5630(3) -0.0426(2) 0.7702(5) 0.027(2) Uani 1 1 d . . . . .
O207 O 0.5691(4) -0.1458(3) 0.6363(6) 0.038(3) Uani 1 1 d . . . . .
O208 O 0.6357(3) -0.1134(2) 0.6222(5) 0.027(2) Uani 1 1 d . . . . .
O209 O 0.6762(3) -0.0423(2) 0.5552(5) 0.032(3) Uani 1 1 d . . . . .
O210 O 0.6196(4) -0.0830(3) 0.5092(5) 0.042(3) Uani 1 1 d . . . . .
O211 O 0.6846(3) 0.0076(2) 0.5546(5) 0.032(3) Uani 1 1 d . . . . .
O212 O 0.6075(3) -0.0095(2) 0.5436(5) 0.032(3) Uani 1 1 d . . . . .
O213 O 0.6259(3) -0.0532(2) 0.6282(5) 0.028(2) Uani 1 1 d . . . . .
O214 O 0.6814(3) -0.0169(2) 0.6851(5) 0.024(2) Uani 1 1 d . . . . .
O215 O 0.6489(3) 0.0287(2) 0.7620(5) 0.028(2) Uani 1 1 d . . . . .
O216 O 0.6073(3) -0.0093(2) 0.6811(5) 0.025(2) Uani 1 1 d . . . . .
O217 O 0.6361(3) -0.0519(2) 0.7648(5) 0.028(2) Uani 1 1 d . . . . .
O218 O 0.5438(3) -0.0419(2) 0.6392(5) 0.031(2) Uani 1 1 d . . . . .
O219 O 0.5802(3) -0.0901(2) 0.6915(5) 0.026(2) Uani 1 1 d . . . . .
O220 O 0.6784(3) -0.2415(2) 0.8252(4) 0.025(2) Uani 1 1 d . . . . .
O221 O 0.8156(7) -0.1717(4) 1.1410(8) 0.092(7) Uani 1 1 d . . . I 1
O222 O 0.7181(10) -0.1510(7) 0.4070(15) 0.152(11) Uiso 1 1 d . . . . .
O223 O 0.7797(7) -0.1140(12) 0.3605(9) 0.24(3) Uani 1 1 d . . . . .
O224 O 0.7144(11) -0.0863(8) 0.3830(17) 0.171(13) Uiso 1 1 d . . . . .
O225 O 0.9011(7) 0.0731(4) 0.9556(9) 0.089(6) Uani 1 1 d . . . . .
O226 O 0.5006(7) 0.1096(6) 0.4461(9) 0.101(7) Uani 1 1 d . . . . .
H226 H 0.522628 0.102288 0.446157 0.152 Uiso 1 1 calc R U . . .
O227 O 0.4567(6) 0.0935(7) 0.5182(12) 0.123(9) Uani 1 1 d . . . . .
O228 O 0.7979(6) 0.0397(4) 0.5432(10) 0.092(6) Uani 1 1 d . . . . .
O229 O 0.5228(6) 0.1533(4) 0.6651(8) 0.080(5) Uani 1 1 d . . . . .
O300 O 0.9105(4) 0.0824(3) 0.1920(5) 0.043(3) Uani 1 1 d . . . J 1
O301 O 0.7076(4) 0.2265(3) 0.9993(6) 0.046(3) Uani 1 1 d . . . . .
O302 O 0.500000 0.000000 0.9501(12) 0.061(6) Uani 1 2 d S T P . .
O303 O 0.3539(4) 0.2584(3) 0.9910(7) 0.060(4) Uani 1 1 d . . . . .
O304 O 0.8793(4) 0.2109(3) 0.1206(7) 0.051(3) Uani 1 1 d . . . . .
O305 O 0.1644(4) 0.2508(3) 0.3739(7) 0.055(4) Uani 1 1 d . . . . .
O306 O 0.6955(5) 0.1288(3) 0.5185(7) 0.060(4) Uani 1 1 d . . . . .
O307 O 0.7085(6) 0.1104(4) 0.3958(8) 0.082(6) Uani 1 1 d . . . . .
O308 O 0.9082(5) 0.1427(4) 0.7002(8) 0.071(5) Uani 1 1 d . . . . .
O309 O 0.9751(5) 0.2614(5) 0.1040(8) 0.087(6) Uani 1 1 d . . . . .
O310 O 0.1103(10) 0.3441(7) 0.9798(16) 0.058(8) Uiso 0.5 1 d . . P K 1
O311 O 0.1304(6) 0.3373(4) 0.5050(9) 0.085(5) Uiso 1 1 d . . . . .
O312 O 0.3881(6) 0.2780(5) 0.7493(10) 0.097(6) Uiso 1 1 d . . . . .
O313 O 0.6538(7) 0.0299(5) 0.3931(10) 0.100(6) Uiso 1 1 d . . . . .
O314 O 0.5900(7) 0.1860(5) 0.7268(11) 0.106(7) Uiso 1 1 d . . . . .
O315 O 0.8277(7) -0.2402(5) 1.2235(11) 0.106(7) Uiso 1 1 d . . . . .
O316 O 0.6647(6) 0.1134(5) 0.0991(10) 0.097(6) Uiso 1 1 d . . . . .
O317 O 0.7612(7) 0.9499(5) 0.7203(11) 0.114(7) Uiso 1 1 d . . . . .
O318 O 0.9298(7) 0.3227(5) 0.9776(11) 0.108(7) Uiso 1 1 d . . . . .
O319 O 0.7994(7) 0.1587(5) 0.2850(11) 0.114(8) Uiso 1 1 d . . . . .
O320 O 0.1604(7) 0.0843(5) 0.0152(11) 0.101(7) Uiso 1 1 d . . . . .
O321 O 0.0251(7) 0.2690(5) 0.4789(10) 0.098(6) Uiso 1 1 d . . . . .
O322 O 0.6365(9) 0.9911(7) 0.0167(14) 0.059(7) Uiso 0.5 1 d . . P . .
O323 O 0.2622(9) 0.1038(6) 0.2374(14) 0.057(7) Uiso 0.5 1 d . . P . .
O324 O 0.1986(9) 0.1499(6) 0.7519(14) 0.056(7) Uiso 0.5 1 d . . P L 1
O325 O 0.1148(8) 0.1785(6) 0.7420(13) 0.051(7) Uiso 0.5 1 d . . P . .
O326 O 0.0754(7) 0.3111(5) 0.4159(10) 0.102(6) Uiso 1 1 d . . . . .
O327 O 1.0152(9) 0.3106(7) 0.0935(14) 0.058(7) Uiso 0.5 1 d . . P . .
O329 O 0.0951(8) 0.1482(6) 0.8522(12) 0.042(6) Uiso 0.5 1 d . . P . .
O330 O 0.1568(10) 0.1097(7) 0.6338(15) 0.064(8) Uiso 0.5 1 d . . P . .
O331 O 0.5806(11) 0.0851(8) 0.4987(17) 0.080(10) Uiso 0.5 1 d . . P . .
O332 O 0.6460(8) 0.1235(6) 0.3173(13) 0.050(7) Uiso 0.5 1 d . . P . .
O333 O 0.4562(8) 0.2501(6) 0.7673(12) 0.047(6) Uiso 0.5 1 d . . P . .
O334 O 0.3828(13) 0.0479(10) 0.407(2) 0.101(13) Uiso 0.5 1 d . . P . .
O335 O 0.8790(9) 0.1717(6) 0.3129(14) 0.055(7) Uiso 0.5 1 d . . P . .
O336 O 0.4492(11) 0.0927(8) 0.0059(17) 0.077(10) Uiso 0.5 1 d . . P . .
O337 O 0.8563(12) 0.3441(9) 0.5002(19) 0.089(11) Uiso 0.5 1 d . . P . .
O338 O 0.1446(10) 0.9682(7) 0.0251(15) 0.063(8) Uiso 0.5 1 d . . P . .
O339 O 0.500000 0.000000 0.8130(19) 0.071(11) Uiso 0.6 2 d S . P . .
O340 O 0.9135(8) 0.7240(6) 0.0948(13) 0.050(7) Uiso 0.5 1 d . . P . .
O341 O 0.1537(10) 0.0687(7) 0.8804(15) 0.066(8) Uiso 0.5 1 d . . P . .
O342 O 0.6311(9) 0.8625(7) 0.1040(15) 0.063(8) Uiso 0.5 1 d . . P . .
O343 O 0.9450(10) 0.8735(8) 0.9935(16) 0.072(9) Uiso 0.5 1 d . . P . .
O344 O 0.7407(11) -0.1831(8) 1.1862(17) 0.082(10) Uiso 0.5 1 d . . P I .
O345 O 0.9822(11) 0.6180(8) 0.7227(16) 0.075(9) Uiso 0.5 1 d . . P . .
O346 O 0.8080(11) 0.8865(8) 0.1781(17) 0.079(10) Uiso 0.5 1 d . . P . .
O347 O 0.3071(11) 0.1495(8) 0.2776(16) 0.075(9) Uiso 0.5 1 d . . P M 1
O348 O 0.4645(12) 0.1978(9) 0.722(2) 0.091(12) Uiso 0.5 1 d . . P N 1
O349 O 0.5805(13) 0.0958(9) 0.3593(19) 0.093(12) Uiso 0.5 1 d . . P . .
O350 O 0.9986(11) 0.3554(8) 0.9950(16) 0.053(9) Uiso 0.4 1 d . . P . .
O351 O 0.5288(14) 0.2735(10) 0.743(2) 0.084(13) Uiso 0.4 1 d . . P . .
O352 O 0.8841(12) -0.1139(9) 0.4550(18) 0.059(10) Uiso 0.4 1 d . . P . .
O353 O 0.9622(14) 0.9311(10) 1.007(2) 0.079(12) Uiso 0.4 1 d . . P . .
O354 O 0.8936(11) 0.0358(8) 0.2236(18) 0.060(10) Uiso 0.4 1 d . . P O 2
O355 O 0.9710(16) 0.3069(12) 0.435(2) 0.093(15) Uiso 0.4 1 d . . P . .
O356 O 0.8728(16) -0.1870(12) 1.255(3) 0.081(14) Uiso 0.35 1 d . . P I .
O358 O 0.5513(15) 0.0375(11) 0.481(2) 0.089(14) Uiso 0.4 1 d . . P P 1
O359 O 0.8383(14) -0.1547(10) 1.327(2) 0.081(13) Uiso 0.4 1 d . . P I .
O360 O 0.8287(14) -0.0350(10) 0.533(2) 0.082(13) Uiso 0.4 1 d . . P . .
O361 O 0.1729(12) 0.1541(9) 0.7156(18) 0.060(10) Uiso 0.4 1 d . . P Q 2
O362 O 0.4652(13) 0.1968(10) 0.783(2) 0.073(12) Uiso 0.4 1 d . . P R 2
O363 O 0.7199(13) -0.1718(10) 1.282(2) 0.075(12) Uiso 0.4 1 d . . P I 2
O364 O 0.1758(15) 0.0920(11) 0.752(2) 0.088(14) Uiso 0.4 1 d . . P . .
O365 O 0.5018(14) 0.0404(10) 0.518(2) 0.081(13) Uiso 0.4 1 d . . P S 2
O366 O 0.1246(10) 0.3431(7) 0.9568(16) 0.041(8) Uiso 0.4 1 d . . P T 2
O367 O 0.7530(14) 0.0362(10) 0.269(2) 0.081(13) Uiso 0.4 1 d . . P . .
O368 O 0.8441(17) 0.0630(12) 0.158(2) 0.096(15) Uiso 0.4 1 d . . P U 1
O369 O 0.383(2) 0.1432(16) 0.234(3) 0.10(2) Uiso 0.3 1 d . . P . .
O370 O 0.0957(15) 0.0277(11) 0.941(2) 0.090(14) Uiso 0.4 1 d . . P . .
O371 O 0.7605(17) -0.0255(12) 1.252(3) 0.071(15) Uiso 0.3 1 d . . P . .
N1 N 0.8907(5) 0.1291(3) 0.8339(7) 0.041(4) Uani 1 1 d . . . . .
H1A H 0.865344 0.133042 0.838643 0.062 Uiso 1 1 calc R U . . .
H1B H 0.897516 0.131614 0.791796 0.062 Uiso 1 1 calc R U . . .
H1C H 0.904554 0.141459 0.859234 0.062 Uiso 1 1 calc R U . . .
N2 N 0.8668(6) 0.0865(5) 0.6414(9) 0.068(6) Uani 1 1 d . . . . .
H2 H 0.855772 0.092092 0.605302 0.081 Uiso 1 1 calc R U . . .
N3 N 0.9892(6) 0.1497(5) 0.8046(8) 0.063(5) Uani 1 1 d . . . . .
H3 H 0.974831 0.156155 0.836453 0.075 Uiso 1 1 calc R U . . .
N4 N 0.9761(12) 0.1429(9) 0.6098(18) 0.160(14) Uiso 1 1 d . . . . .
H4A H 0.972176 0.139444 0.652560 0.240 Uiso 1 1 calc R U . . .
H4B H 0.963525 0.129252 0.585914 0.240 Uiso 1 1 calc R U . . .
H4C H 0.967184 0.161082 0.599562 0.240 Uiso 1 1 calc R U . . .
N5 N 0.7749(5) -0.0389(3) 0.8568(7) 0.042(4) Uani 1 1 d . . . . .
H5A H 0.796397 -0.049515 0.865256 0.063 Uiso 1 1 calc R U . . .
H5B H 0.772991 -0.035852 0.813421 0.063 Uiso 1 1 calc R U . . .
H5C H 0.754025 -0.048980 0.870816 0.063 Uiso 1 1 calc R U . . .
N6 N 0.7990(6) 0.0223(4) 0.6932(8) 0.059(5) Uani 1 1 d . . . . .
H6 H 0.785195 0.027679 0.659720 0.071 Uiso 1 1 calc R U . . .
N7 N 0.5240(7) 0.1633(4) 0.7908(9) 0.074(6) Uani 1 1 d . . . . .
H7A H 0.501824 0.171753 0.777058 0.111 Uiso 1 1 calc R U . . .
H7B H 0.542959 0.167245 0.761954 0.111 Uiso 1 1 calc R U . . .
H7C H 0.530417 0.170725 0.830168 0.111 Uiso 1 1 calc R U . . .
N8 N 0.5431(7) 0.1381(5) 0.5317(9) 0.076(6) Uani 1 1 d . . . . .
H8A H 0.562972 0.126690 0.544748 0.113 Uiso 1 1 calc R U . . .
H8B H 0.545717 0.156372 0.548982 0.113 Uiso 1 1 calc R U . . .
H8C H 0.543073 0.139418 0.487818 0.113 Uiso 1 1 calc R U . . .
C1 C 0.8920(8) 0.0971(5) 0.9273(11) 0.063(6) Uani 1 1 d . . . . .
C2 C 0.8981(7) 0.0992(5) 0.8529(11) 0.059(6) Uani 1 1 d . . . . .
H2A H 0.925440 0.094506 0.842994 0.070 Uiso 1 1 calc R U . . .
C3 C 0.8710(9) 0.0753(6) 0.8177(12) 0.075(7) Uani 1 1 d . . . . .
H3A H 0.877310 0.055370 0.833489 0.090 Uiso 1 1 calc R U . . .
H3B H 0.843838 0.079296 0.827764 0.090 Uiso 1 1 calc R U . . .
C4 C 0.8775(8) 0.0770(5) 0.7452(11) 0.065(6) Uani 1 1 d . . . . .
C5 C 0.8497(10) 0.0862(6) 0.6971(15) 0.085(9) Uani 1 1 d . . . . .
H5 H 0.823716 0.091055 0.704882 0.102 Uiso 1 1 calc R U . . .
C6 C 0.9048(8) 0.0768(6) 0.6450(12) 0.075(8) Uani 1 1 d . . . . .
C7 C 0.9125(8) 0.0723(6) 0.7111(12) 0.075(8) Uani 1 1 d . . . . .
C8 C 0.9501(10) 0.0639(7) 0.7295(14) 0.099(11) Uani 1 1 d . . . . .
H8 H 0.956531 0.060271 0.773369 0.119 Uiso 1 1 calc R U . . .
C9 C 0.9781(13) 0.0611(9) 0.6782(19) 0.123(13) Uiso 1 1 d . . . . .
H9 H 1.003799 0.056400 0.689334 0.147 Uiso 1 1 calc R U . . .
C10 C 0.9688(12) 0.0650(8) 0.6130(19) 0.116(12) Uiso 1 1 d . . . . .
H10 H 0.987947 0.062935 0.580731 0.139 Uiso 1 1 calc R U . . .
C11 C 0.9305(10) 0.0721(7) 0.5949(17) 0.099(10) Uiso 1 1 d . . . . .
H11 H 0.922972 0.073474 0.550849 0.118 Uiso 1 1 calc R U . . .
C12 C 1.0277(7) 0.1601(7) 0.5300(10) 0.072(8) Uani 1 1 d . . . . .
C13 C 1.0179(8) 0.1414(6) 0.5954(16) 0.091(10) Uani 1 1 d . . . . .
H13 H 1.028206 0.120960 0.594724 0.109 Uiso 1 1 calc R U . . .
C14 C 1.0411(12) 0.1623(9) 0.6381(17) 0.118(12) Uiso 1 1 d . . . . .
H14A H 1.034625 0.183124 0.629993 0.141 Uiso 1 1 calc R U . . .
H14B H 1.068989 0.159330 0.633587 0.141 Uiso 1 1 calc R U . . .
C15 C 1.0237(9) 0.1499(7) 0.7121(14) 0.039(7) Uiso 0.6 1 d . . P . .
C16 C 0.9935(7) 0.1626(6) 0.7491(12) 0.068(6) Uiso 1 1 d . . . . .
H16 H 0.978330 0.178621 0.734841 0.081 Uiso 1 1 calc R U . . .
C17 C 1.0301(9) 0.1241(7) 0.7479(15) 0.085(8) Uiso 1 1 d . . . . .
C18 C 1.0097(9) 0.1256(7) 0.8060(14) 0.079(8) Uiso 1 1 d . . . . .
C19 C 1.016(2) 0.1079(15) 0.861(3) 0.20(3) Uiso 1 1 d . . . . .
H19 H 1.005387 0.111414 0.902644 0.246 Uiso 1 1 calc R U . . .
C20 C 1.038(2) 0.0856(15) 0.846(3) 0.20(3) Uiso 1 1 d . . . . .
H20 H 1.037686 0.069811 0.875473 0.239 Uiso 1 1 calc R U . . .
C21 C 1.0618(15) 0.0814(11) 0.795(2) 0.142(16) Uiso 1 1 d . . . . .
H21 H 1.080073 0.066021 0.794848 0.170 Uiso 1 1 calc R U . . .
C22 C 1.0587(12) 0.1015(9) 0.738(2) 0.128(13) Uiso 1 1 d . . . . .
H22 H 1.073702 0.099745 0.700129 0.153 Uiso 1 1 calc R U . . .
C23 C 0.7765(5) -0.0151(4) 0.9634(9) 0.037(4) Uani 1 1 d . . . . .
C24 C 0.7770(5) -0.0109(4) 0.8900(9) 0.041(4) Uani 1 1 d . . . . .
H24 H 0.754361 0.001140 0.877342 0.049 Uiso 1 1 calc R U . . .
C25 C 0.8139(6) 0.0054(4) 0.8686(9) 0.046(5) Uani 1 1 d . . . . .
H25A H 0.836491 -0.006209 0.881600 0.056 Uiso 1 1 calc R U . . .
H25B H 0.815221 0.024508 0.891319 0.056 Uiso 1 1 calc R U . . .
C26 C 0.8153(5) 0.0109(4) 0.7941(8) 0.038(4) Uani 1 1 d . . . . .
C27 C 0.7874(7) 0.0226(5) 0.7570(11) 0.058(5) Uani 1 1 d . . . . .
H27 H 0.763604 0.029788 0.772337 0.070 Uiso 1 1 calc R U . . .
C28 C 0.8463(7) 0.0040(5) 0.7554(11) 0.065(7) Uani 1 1 d . . . . .
C29 C 0.8360(8) 0.0122(6) 0.6914(11) 0.070(7) Uani 1 1 d . . . . .
C30 C 0.8620(11) 0.0119(7) 0.6384(16) 0.102(11) Uani 1 1 d . . . . .
H30 H 0.855355 0.019336 0.596953 0.122 Uiso 1 1 calc R U . . .
C31 C 0.8981(10) -0.0002(8) 0.6518(14) 0.099(11) Uani 1 1 d . . . . .
H31 H 0.915774 -0.004005 0.617903 0.119 Uiso 1 1 calc R U . . .
C32 C 0.9070(13) -0.0061(8) 0.7129(18) 0.116(12) Uiso 1 1 d . . . . .
H32 H 0.933243 -0.009344 0.722418 0.139 Uiso 1 1 calc R U . . .
C33 C 0.8812(11) -0.0080(8) 0.7645(18) 0.105(10) Uiso 1 1 d . . . . .
H33 H 0.887892 -0.017195 0.804038 0.126 Uiso 1 1 calc R U . . .
C34 C 0.4855(8) 0.1074(8) 0.5045(13) 0.081(9) Uani 1 1 d . . . . .
C35 C 0.5054(8) 0.1246(6) 0.5546(11) 0.068(7) Uani 1 1 d . . . . .
H35 H 0.488175 0.141341 0.565826 0.082 Uiso 1 1 calc R U . . .
C36 C 0.5112(6) 0.1070(5) 0.6171(9) 0.046(5) Uani 1 1 d . . . . .
H36A H 0.488452 0.094605 0.624884 0.055 Uiso 1 1 calc R U . . .
H36B H 0.533630 0.093957 0.612076 0.055 Uiso 1 1 calc R U . . .
C37 C 0.5174(6) 0.1270(5) 0.6744(11) 0.054(5) Uani 1 1 d . . . . .
C39 C 0.5188(6) 0.1324(5) 0.7958(11) 0.057(6) Uani 1 1 d . . . . .
C40 C 0.5167(5) 0.1146(4) 0.7381(10) 0.045(4) Uani 1 1 d . . . . .
C41 C 0.5133(5) 0.0832(4) 0.7473(11) 0.048(5) Uani 1 1 d . . . . .
H41 H 0.512661 0.070570 0.710855 0.058 Uiso 1 1 calc R U . . .
C42 C 0.5110(6) 0.0715(5) 0.8094(10) 0.049(5) Uani 1 1 d . . . . .
H42 H 0.508263 0.050935 0.815383 0.058 Uiso 1 1 calc R U . . .
C43 C 0.5129(6) 0.0903(5) 0.8633(11) 0.058(6) Uani 1 1 d . . . . .
H43 H 0.511419 0.082049 0.905354 0.069 Uiso 1 1 calc R U . . .
C44 C 0.5167(7) 0.1208(5) 0.8573(11) 0.057(6) Uani 1 1 d . . . . .
H44 H 0.517803 0.133003 0.894361 0.069 Uiso 1 1 calc R U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O17 Mo1 O10 103.1(5) . .
O17 Mo1 O14 98.4(5) . .
O10 Mo1 O14 89.6(4) . .
O17 Mo1 O7 102.0(5) . .
O10 Mo1 O7 87.3(4) . .
O14 Mo1 O7 159.5(4) . .
O17 Mo1 O19 101.1(5) . .
O10 Mo1 O19 155.7(4) . .
O14 Mo1 O19 88.9(4) . .
O7 Mo1 O19 85.7(4) . .
O17 Mo1 O18 167.4(4) . .
O10 Mo1 O18 87.0(4) . .
O14 Mo1 O18 74.0(4) . .
O7 Mo1 O18 85.7(4) . .
O19 Mo1 O18 69.3(4) . .
O33 Mo2 O35 103.1(5) . .
O33 Mo2 O32 99.7(5) . .
O35 Mo2 O32 88.7(4) . .
O33 Mo2 O34 102.2(5) . .
O35 Mo2 O34 87.3(4) . .
O32 Mo2 O34 158.0(4) . .
O33 Mo2 O19 97.6(5) . .
O35 Mo2 O19 159.2(4) . .
O32 Mo2 O19 89.9(4) . .
O34 Mo2 O19 86.4(4) . .
O33 Mo2 O30 168.0(5) . .
O35 Mo2 O30 88.0(4) . .
O32 Mo2 O30 75.5(4) . .
O34 Mo2 O30 82.7(4) . .
O19 Mo2 O30 71.6(4) . .
O27 Mo3 O36 102.5(5) . .
O27 Mo3 O32 102.9(5) . .
O36 Mo3 O32 98.0(4) . .
O27 Mo3 O28 104.2(5) . .
O36 Mo3 O28 87.1(4) . .
O32 Mo3 O28 150.6(4) . .
O27 Mo3 O26 96.5(5) . .
O36 Mo3 O26 155.3(4) . .
O32 Mo3 O26 93.0(4) . .
O28 Mo3 O26 72.9(4) . .
O27 Mo3 O30 170.1(4) . .
O36 Mo3 O30 87.3(4) . .
O32 Mo3 O30 73.6(4) . .
O28 Mo3 O30 77.7(4) . .
O26 Mo3 O30 74.6(4) . .
O52 Mo4 O36 103.6(5) . .
O52 Mo4 O51 97.0(4) . .
O36 Mo4 O51 89.6(4) . .
O52 Mo4 O45 102.3(5) . .
O36 Mo4 O45 87.0(4) . .
O51 Mo4 O45 160.7(4) . .
O52 Mo4 O61 99.0(5) . .
O36 Mo4 O61 157.3(4) . .
O51 Mo4 O61 88.0(4) . .
O45 Mo4 O61 87.8(4) . .
O52 Mo4 O50 167.1(5) . .
O36 Mo4 O50 86.7(4) . .
O51 Mo4 O50 75.0(4) . .
O45 Mo4 O50 85.8(4) . .
O61 Mo4 O50 70.9(4) . .
O54 Mo5 O35 102.5(5) . .
O54 Mo5 O51 103.7(5) . .
O35 Mo5 O51 99.2(4) . .
O54 Mo5 O53 104.3(5) . .
O35 Mo5 O53 87.5(4) . .
O51 Mo5 O53 149.0(4) . .
O54 Mo5 O68 96.6(5) . .
O35 Mo5 O68 155.0(4) . .
O51 Mo5 O68 91.7(4) . .
O53 Mo5 O68 72.1(4) . .
O54 Mo5 O50 170.0(4) . .
O35 Mo5 O50 87.1(4) . .
O51 Mo5 O50 71.6(4) . .
O53 Mo5 O50 78.6(4) . .
O68 Mo5 O50 75.0(4) . .
O71 Mo6 O94 102.4(5) . .
O71 Mo6 O65 102.3(5) . .
O94 Mo6 O65 99.8(4) . .
O71 Mo6 O70 105.0(5) . .
O94 Mo6 O70 87.5(4) . .
O65 Mo6 O70 149.4(4) . .
O71 Mo6 O68 94.9(5) . .
O94 Mo6 O68 155.9(4) . .
O65 Mo6 O68 92.7(4) . .
O70 Mo6 O68 71.7(4) . .
O71 Mo6 O66 168.6(5) . .
O94 Mo6 O66 88.8(4) . .
O65 Mo6 O66 73.2(4) . .
O70 Mo6 O66 77.4(4) . .
O68 Mo6 O66 75.1(4) . .
O62 Mo7 O63 103.2(5) . .
O62 Mo7 O65 99.7(5) . .
O63 Mo7 O65 88.5(5) . .
O62 Mo7 O64 103.6(5) . .
O63 Mo7 O64 87.7(5) . .
O65 Mo7 O64 156.7(4) . .
O62 Mo7 O61 99.3(5) . .
O63 Mo7 O61 157.5(4) . .
O65 Mo7 O61 88.0(4) . .
O64 Mo7 O61 86.8(5) . .
O62 Mo7 O66 168.1(5) . .
O63 Mo7 O66 86.9(4) . .
O65 Mo7 O66 73.9(4) . .
O64 Mo7 O66 82.9(4) . .
O61 Mo7 O66 70.8(4) . .
O95 Mo8 O94 103.8(5) . .
O95 Mo8 O92 99.1(5) . .
O94 Mo8 O92 89.0(4) . .
O95 Mo8 O93 102.2(5) . .
O94 Mo8 O93 86.8(4) . .
O92 Mo8 O93 158.7(4) . .
O95 Mo8 O114 101.4(5) . .
O94 Mo8 O114 154.7(4) . .
O92 Mo8 O114 88.7(4) . .
O93 Mo8 O114 86.3(4) . .
O95 Mo8 O91 167.9(5) . .
O94 Mo8 O91 86.2(4) . .
O92 Mo8 O91 73.9(4) . .
O93 Mo8 O91 85.0(4) . .
O114 Mo8 O91 69.0(4) . .
O133 Mo9 O125 102.7(5) . .
O133 Mo9 O131 102.3(5) . .
O125 Mo9 O131 96.9(4) . .
O133 Mo9 O124 103.7(5) . .
O125 Mo9 O124 88.3(4) . .
O131 Mo9 O124 151.6(4) . .
O133 Mo9 O155 96.8(5) . .
O125 Mo9 O155 155.0(4) . .
O131 Mo9 O155 93.9(4) . .
O124 Mo9 O155 71.9(4) . .
O133 Mo9 O132 170.6(5) . .
O125 Mo9 O132 86.3(4) . .
O131 Mo9 O132 73.6(4) . .
O124 Mo9 O132 79.0(4) . .
O155 Mo9 O132 75.3(4) . .
O151 Mo10 O140 103.8(5) . .
O151 Mo10 O153 104.5(5) . .
O140 Mo10 O153 100.9(5) . .
O151 Mo10 O132 102.7(5) . .
O140 Mo10 O132 97.1(4) . .
O153 Mo10 O132 142.5(4) . .
O151 Mo10 O152 100.3(4) . .
O140 Mo10 O152 155.7(4) . .
O153 Mo10 O152 76.0(4) . .
O132 Mo10 O152 74.2(4) . .
O151 Mo10 O155 177.1(4) . .
O140 Mo10 O155 73.9(4) . .
O153 Mo10 O155 77.8(4) . .
O132 Mo10 O155 76.0(4) . .
O152 Mo10 O155 81.9(3) . .
O130 Mo11 O110 104.6(5) . .
O130 Mo11 O131 100.9(5) . .
O110 Mo11 O131 91.4(4) . .
O130 Mo11 O129 102.5(5) . .
O110 Mo11 O129 85.9(4) . .
O131 Mo11 O129 156.4(4) . .
O130 Mo11 O152 101.5(5) . .
O110 Mo11 O152 153.5(4) . .
O131 Mo11 O152 88.1(4) . .
O129 Mo11 O152 84.1(4) . .
O130 Mo11 O132 169.2(5) . .
O110 Mo11 O132 85.1(4) . .
O131 Mo11 O132 73.5(4) . .
O129 Mo11 O132 82.9(4) . .
O152 Mo11 O132 69.4(4) . .
O177 Mo12 O220 103.7(5) . .
O177 Mo12 O178 102.0(5) . .
O220 Mo12 O178 94.8(4) . .
O177 Mo12 O167 104.7(5) . .
O220 Mo12 O167 89.1(4) . .
O178 Mo12 O167 151.3(4) . .
O177 Mo12 O176 96.8(5) . .
O220 Mo12 O176 155.2(4) . .
O178 Mo12 O176 94.5(4) . .
O167 Mo12 O176 72.0(4) . .
O177 Mo12 O166 170.7(4) . .
O220 Mo12 O166 84.9(4) . .
O178 Mo12 O166 73.4(4) . .
O167 Mo12 O166 78.7(4) . .
O176 Mo12 O166 75.8(4) . .
O201 Mo13 O204 103.4(5) . .
O201 Mo13 O203 102.6(5) . .
O204 Mo13 O203 97.1(5) . .
O201 Mo13 O174 102.9(5) . .
O204 Mo13 O174 89.1(5) . .
O203 Mo13 O174 151.5(4) . .
O201 Mo13 O176 96.1(5) . .
O204 Mo13 O176 155.5(4) . .
O203 Mo13 O176 93.0(4) . .
O174 Mo13 O176 71.9(4) . .
O201 Mo13 O194 170.9(5) . .
O204 Mo13 O194 85.6(4) . .
O203 Mo13 O194 74.1(4) . .
O174 Mo13 O194 78.8(4) . .
O176 Mo13 O194 75.8(3) . .
O207 Mo14 O219 104.2(5) . .
O207 Mo14 O203 99.9(5) . .
O219 Mo14 O203 91.9(4) . .
O207 Mo14 O208 100.0(5) . .
O219 Mo14 O208 86.6(4) . .
O203 Mo14 O208 159.7(5) . .
O207 Mo14 O193 101.8(5) . .
O219 Mo14 O193 153.5(4) . .
O203 Mo14 O193 88.2(4) . .
O208 Mo14 O193 84.3(4) . .
O207 Mo14 O194 168.4(5) . .
O219 Mo14 O194 85.8(4) . .
O203 Mo14 O194 73.6(4) . .
O208 Mo14 O194 86.2(4) . .
O193 Mo14 O194 68.9(4) . .
O202 Mo15 O204 102.9(5) . .
O202 Mo15 O206 99.4(5) . .
O204 Mo15 O206 91.0(5) . .
O202 Mo15 O190 100.1(5) . .
O204 Mo15 O190 86.5(5) . .
O206 Mo15 O190 160.4(4) . .
O202 Mo15 O205 101.0(5) . .
O204 Mo15 O205 155.8(4) . .
O206 Mo15 O205 88.4(4) . .
O190 Mo15 O205 86.0(4) . .
O202 Mo15 O217 167.6(5) . .
O204 Mo15 O217 87.9(4) . .
O206 Mo15 O217 74.0(4) . .
O190 Mo15 O217 86.5(4) . .
O205 Mo15 O217 68.7(4) . .
O9 Mo18 O11 103.8(5) . .
O9 Mo18 O10 102.0(5) . .
O11 Mo18 O10 99.2(4) . .
O9 Mo18 O8 105.0(5) . .
O11 Mo18 O8 148.4(4) . .
O10 Mo18 O8 87.5(4) . .
O9 Mo18 O216 96.8(5) . .
O11 Mo18 O216 91.7(4) . .
O10 Mo18 O216 155.3(4) . .
O8 Mo18 O216 72.2(4) . .
O9 Mo18 O215 171.1(5) . .
O11 Mo18 O215 71.9(4) . .
O10 Mo18 O215 86.5(4) . .
O8 Mo18 O215 77.7(4) . .
O216 Mo18 O215 75.8(4) . .
O90 Mo19 O63 104.3(5) . .
O90 Mo19 O92 101.7(5) . .
O63 Mo19 O92 99.7(5) . .
O90 Mo19 O89 105.9(5) . .
O63 Mo19 O89 86.8(5) . .
O92 Mo19 O89 149.2(4) . .
O90 Mo19 O101 95.4(5) . .
O63 Mo19 O101 154.6(4) . .
O92 Mo19 O101 91.8(4) . .
O89 Mo19 O101 72.3(4) . .
O90 Mo19 O91 167.5(5) . .
O63 Mo19 O91 87.8(4) . .
O92 Mo19 O91 72.7(4) . .
O89 Mo19 O91 77.5(4) . .
O101 Mo19 O91 73.9(4) . .
O157 Mo20 O163 103.4(5) . .
O157 Mo20 O154 99.9(5) . .
O163 Mo20 O154 94.7(4) . .
O157 Mo20 O156 103.3(5) . .
O163 Mo20 O156 89.8(4) . .
O154 Mo20 O156 154.6(4) . .
O157 Mo20 O155 94.0(5) . .
O163 Mo20 O155 157.8(4) . .
O154 Mo20 O155 95.9(4) . .
O156 Mo20 O155 72.6(4) . .
O157 Mo20 O153 168.5(5) . .
O163 Mo20 O153 87.4(4) . .
O154 Mo20 O153 75.0(4) . .
O156 Mo20 O153 80.3(4) . .
O155 Mo20 O153 76.6(4) . .
O80 Mo21 O96 103.8(5) . .
O80 Mo21 O93 100.6(5) . .
O96 Mo21 O93 106.1(5) . .
O80 Mo21 O75 96.3(5) . .
O96 Mo21 O75 88.5(4) . .
O93 Mo21 O75 154.2(4) . .
O80 Mo21 O70 95.8(5) . .
O96 Mo21 O70 151.4(4) . .
O93 Mo21 O70 90.2(4) . .
O75 Mo21 O70 68.6(4) . .
O80 Mo21 O79 170.3(5) . .
O96 Mo21 O79 82.6(5) . .
O93 Mo21 O79 84.4(4) . .
O75 Mo21 O79 76.4(4) . .
O70 Mo21 O79 75.7(4) . .
O109 Mo22 O112 103.3(5) . .
O109 Mo22 O110 103.9(5) . 2_755
O112 Mo22 O110 96.7(5) . 2_755
O109 Mo22 O108 103.7(5) . .
O112 Mo22 O108 150.4(4) . .
O110 Mo22 O108 88.6(4) 2_755 .
O109 Mo22 O101 95.1(5) . .
O112 Mo22 O101 94.0(4) . .
O110 Mo22 O101 155.4(4) 2_755 .
O108 Mo22 O101 71.6(4) . .
O109 Mo22 O111 167.8(4) . .
O112 Mo22 O111 71.9(4) . .
O110 Mo22 O111 87.9(4) 2_755 .
O108 Mo22 O111 79.2(4) . .
O101 Mo22 O111 74.4(4) . .
O150 Mo23 O220 104.5(5) . .
O150 Mo23 O154 98.6(5) . .
O220 Mo23 O154 93.3(4) . .
O150 Mo23 O149 101.5(5) . .
O220 Mo23 O149 86.8(4) . .
O154 Mo23 O149 159.2(4) . .
O150 Mo23 O152 101.0(5) . .
O220 Mo23 O152 154.3(4) . .
O154 Mo23 O152 86.6(4) . .
O149 Mo23 O152 84.4(4) . .
O150 Mo23 O153 167.1(4) . .
O220 Mo23 O153 86.3(4) . .
O154 Mo23 O153 73.2(4) . .
O149 Mo23 O153 86.0(4) . .
O152 Mo23 O153 69.0(4) . .
O179 Mo24 O175 102.6(5) . .
O179 Mo24 O194 104.8(5) . .
O175 Mo24 O194 103.1(5) . .
O179 Mo24 O166 103.0(5) . .
O175 Mo24 O166 95.6(4) . .
O194 Mo24 O166 142.0(4) . .
O179 Mo24 O193 101.2(5) . .
O175 Mo24 O193 155.4(4) . .
O194 Mo24 O193 76.7(4) . .
O166 Mo24 O193 72.8(4) . .
O179 Mo24 O176 176.4(4) . .
O175 Mo24 O176 74.4(4) . .
O194 Mo24 O176 78.1(4) . .
O166 Mo24 O176 75.5(4) . .
O193 Mo24 O176 81.6(4) . .
O138 Mo25 O134 99.2(5) . .
O138 Mo25 O124 96.2(5) . .
O134 Mo25 O124 72.6(4) . .
O138 Mo25 O137 102.3(5) . .
O134 Mo25 O137 71.0(4) . .
O124 Mo25 O137 141.1(4) . .
O138 Mo25 O156 93.6(5) . .
O134 Mo25 O156 142.5(4) . .
O124 Mo25 O156 140.9(4) . .
O137 Mo25 O156 71.9(4) . .
O138 Mo25 O155 95.8(4) . .
O134 Mo25 O155 141.4(4) . .
O124 Mo25 O155 70.6(4) . .
O137 Mo25 O155 139.4(4) . .
O156 Mo25 O155 70.9(4) . .
O138 Mo25 O140 168.7(4) . .
O134 Mo25 O140 90.6(4) . .
O124 Mo25 O140 81.2(4) . .
O137 Mo25 O140 86.2(4) . .
O156 Mo25 O140 81.9(4) . .
O155 Mo25 O140 73.0(4) . .
O126 Mo26 O128 105.1(5) . .
O126 Mo26 O129 102.6(5) . 2_755
O128 Mo26 O129 104.6(5) . 2_755
O126 Mo26 O106 94.6(5) . .
O128 Mo26 O106 91.9(5) . .
O129 Mo26 O106 151.9(5) 2_755 .
O126 Mo26 O108 94.8(5) . .
O128 Mo26 O108 153.2(4) . .
O129 Mo26 O108 87.9(4) 2_755 .
O106 Mo26 O108 68.4(4) . .
O126 Mo26 O127 172.5(5) . .
O128 Mo26 O127 81.4(5) . .
O129 Mo26 O127 79.0(4) 2_755 .
O106 Mo26 O127 81.3(4) . .
O108 Mo26 O127 77.8(4) . .
O72 Mo27 O73 99.6(5) . .
O72 Mo27 O75 101.9(5) . .
O73 Mo27 O75 71.2(4) . .
O72 Mo27 O70 93.8(5) . .
O73 Mo27 O70 142.8(4) . .
O75 Mo27 O70 72.1(4) . .
O72 Mo27 O53 93.5(5) . .
O73 Mo27 O53 71.1(4) . .
O75 Mo27 O53 141.1(4) . .
O70 Mo27 O53 142.7(4) . .
O72 Mo27 O68 96.8(4) . .
O73 Mo27 O68 139.7(4) . .
O75 Mo27 O68 139.9(4) . .
O70 Mo27 O68 71.5(4) . .
O53 Mo27 O68 71.3(4) . .
O72 Mo27 O69 171.8(4) . .
O73 Mo27 O69 87.2(4) . .
O75 Mo27 O69 84.6(4) . .
O70 Mo27 O69 83.4(4) . .
O53 Mo27 O69 84.2(4) . .
O68 Mo27 O69 75.0(4) . .
O55 Mo28 O57 104.4(5) . .
O55 Mo28 O34 101.7(5) . .
O57 Mo28 O34 106.8(5) . .
O55 Mo28 O73 97.8(5) . .
O57 Mo28 O73 87.4(5) . .
O34 Mo28 O73 152.0(4) . .
O55 Mo28 O53 95.1(5) . .
O57 Mo28 O53 150.4(5) . .
O34 Mo28 O53 90.4(4) . .
O73 Mo28 O53 67.8(4) . .
O55 Mo28 O56 174.2(5) . .
O57 Mo28 O56 80.9(5) . .
O34 Mo28 O56 78.6(4) . .
O73 Mo28 O56 80.0(4) . .
O53 Mo28 O56 79.1(4) . .
O165 Mo29 O163 102.8(5) . .
O165 Mo29 O178 99.2(5) . .
O163 Mo29 O178 93.5(4) . .
O165 Mo29 O164 102.3(5) . .
O163 Mo29 O164 86.8(4) . .
O178 Mo29 O164 157.9(5) . .
O165 Mo29 O193 102.4(5) . .
O163 Mo29 O193 154.3(4) . .
O178 Mo29 O193 87.3(4) . .
O164 Mo29 O193 83.1(4) . .
O165 Mo29 O166 168.4(5) . .
O163 Mo29 O166 86.9(4) . .
O178 Mo29 O166 73.7(4) . .
O164 Mo29 O166 84.3(4) . .
O193 Mo29 O166 68.7(4) . .
O148 Mo30 O146 104.0(6) . .
O148 Mo30 O149 102.0(5) . .
O146 Mo30 O149 103.9(5) . .
O148 Mo30 O168 91.3(5) . .
O146 Mo30 O168 91.9(5) . .
O149 Mo30 O168 156.0(5) . .
O148 Mo30 O167 95.4(5) . .
O146 Mo30 O167 152.4(5) . .
O149 Mo30 O167 90.9(4) . .
O168 Mo30 O167 67.9(4) . .
O148 Mo30 O147 169.2(5) . .
O146 Mo30 O147 83.9(5) . .
O149 Mo30 O147 83.0(5) . .
O168 Mo30 O147 80.9(4) . .
O167 Mo30 O147 74.8(4) . .
O218 Mo31 O219 102.4(5) . .
O218 Mo31 O206 103.8(5) . .
O219 Mo31 O206 96.6(4) . .
O218 Mo31 O213 105.6(5) . .
O219 Mo31 O213 87.9(4) . .
O206 Mo31 O213 148.5(4) . .
O218 Mo31 O216 97.2(5) . .
O219 Mo31 O216 155.2(4) . .
O206 Mo31 O216 93.3(4) . .
O213 Mo31 O216 72.2(4) . .
O218 Mo31 O217 170.2(4) . .
O219 Mo31 O217 86.7(4) . .
O206 Mo31 O217 71.2(4) . .
O213 Mo31 O217 78.0(4) . .
O216 Mo31 O217 75.0(4) . .
O67 Mo32 O69 103.3(5) . .
O67 Mo32 O66 107.1(5) . .
O69 Mo32 O66 99.6(5) . .
O67 Mo32 O50 103.8(5) . .
O69 Mo32 O50 96.1(4) . .
O66 Mo32 O50 140.8(4) . .
O67 Mo32 O61 98.9(5) . .
O69 Mo32 O61 157.3(4) . .
O66 Mo32 O61 78.1(4) . .
O50 Mo32 O61 73.8(4) . .
O67 Mo32 O68 175.3(4) . .
O69 Mo32 O68 72.5(4) . .
O66 Mo32 O68 76.1(4) . .
O50 Mo32 O68 74.8(4) . .
O61 Mo32 O68 85.2(4) . .
O103 Mo33 O106 99.3(5) . .
O103 Mo33 O88 102.1(5) . .
O106 Mo33 O88 72.0(4) . .
O103 Mo33 O108 93.7(5) . .
O106 Mo33 O108 72.5(4) . .
O88 Mo33 O108 143.0(4) . .
O103 Mo33 O89 93.6(5) . .
O106 Mo33 O89 143.3(4) . .
O88 Mo33 O89 71.7(4) . .
O108 Mo33 O89 141.0(4) . .
O103 Mo33 O101 98.7(5) . .
O106 Mo33 O101 139.4(4) . .
O88 Mo33 O101 137.8(4) . .
O108 Mo33 O101 70.3(4) . .
O89 Mo33 O101 70.7(4) . .
O103 Mo33 O102 171.8(5) . .
O106 Mo33 O102 87.7(4) . .
O88 Mo33 O102 84.1(4) . .
O108 Mo33 O102 84.3(4) . .
O89 Mo33 O102 83.0(4) . .
O101 Mo33 O102 73.1(4) . .
O191 Mo34 O214 103.3(5) . .
O191 Mo34 O215 105.5(5) . .
O214 Mo34 O215 102.3(4) . .
O191 Mo34 O217 104.8(5) . .
O214 Mo34 O217 93.9(4) . .
O215 Mo34 O217 140.9(4) . .
O191 Mo34 O205 99.9(5) . .
O214 Mo34 O205 155.7(4) . .
O215 Mo34 O205 77.7(4) . .
O217 Mo34 O205 73.4(4) . .
O40 Mo35 O41 102.5(6) . .
O40 Mo35 O39 104.5(6) . .
O41 Mo35 O39 104.5(5) . .
O40 Mo35 O37 96.9(5) . .
O41 Mo35 O37 90.1(5) . .
O39 Mo35 O37 150.7(5) . .
O40 Mo35 O25 97.6(5) . .
O41 Mo35 O25 152.9(5) . .
O39 Mo35 O25 87.7(5) . .
O37 Mo35 O25 69.4(4) . .
O40 Mo35 O38 171.7(5) . .
O41 Mo35 O38 79.6(5) . .
O39 Mo35 O38 82.5(5) . .
O37 Mo35 O38 75.1(4) . .
O25 Mo35 O38 78.1(4) . .
O113 Mo36 O102 104.1(5) . .
O113 Mo36 O111 106.0(5) . .
O102 Mo36 O111 99.1(4) . .
O113 Mo36 O91 104.8(5) . .
O102 Mo36 O91 96.3(4) . .
O111 Mo36 O91 140.8(4) . .
O113 Mo36 O114 98.5(5) . .
O102 Mo36 O114 157.2(4) . .
O111 Mo36 O114 77.3(4) . .
O91 Mo36 O114 74.6(4) . .
O113 Mo36 O101 176.0(5) . .
O102 Mo36 O101 72.4(4) . .
O111 Mo36 O101 76.6(4) . .
O91 Mo36 O101 74.2(4) . .
O114 Mo36 O101 84.9(4) . .
O21 Mo37 O22 105.1(6) . .
O21 Mo37 O15 100.5(5) . .
O22 Mo37 O15 105.4(5) . .
O21 Mo37 O25 95.0(5) . .
O22 Mo37 O25 88.7(5) . .
O15 Mo37 O25 155.3(5) . .
O21 Mo37 O20 93.4(5) . .
O22 Mo37 O20 151.3(5) . .
O15 Mo37 O20 92.2(5) . .
O25 Mo37 O20 67.7(4) . .
O21 Mo37 O23 171.1(5) . .
O22 Mo37 O23 82.9(6) . .
O15 Mo37 O23 80.4(5) . .
O25 Mo37 O23 81.4(4) . .
O20 Mo37 O23 77.7(4) . .
O24 Mo38 O25 98.8(5) . .
O24 Mo38 O20 95.5(5) . .
O25 Mo38 O20 71.5(4) . .
O24 Mo38 O37 103.1(5) . .
O25 Mo38 O37 71.8(5) . .
O20 Mo38 O37 140.8(4) . .
O24 Mo38 O28 91.7(5) . .
O25 Mo38 O28 142.6(4) . .
O20 Mo38 O28 143.3(4) . .
O37 Mo38 O28 70.9(4) . .
O24 Mo38 O26 95.8(5) . .
O25 Mo38 O26 140.9(4) . .
O20 Mo38 O26 71.2(4) . .
O37 Mo38 O26 138.8(4) . .
O28 Mo38 O26 72.4(4) . .
O24 Mo38 O29 170.6(5) . .
O25 Mo38 O29 89.5(4) . .
O20 Mo38 O29 82.7(4) . .
O37 Mo38 O29 83.8(4) . .
O28 Mo38 O29 84.5(4) . .
O26 Mo38 O29 74.8(4) . .
O43 Mo39 O42 105.0(6) . .
O43 Mo39 O45 101.3(5) . .
O42 Mo39 O45 104.9(5) . .
O43 Mo39 O37 95.2(5) . .
O42 Mo39 O37 89.8(5) . .
O45 Mo39 O37 154.1(5) . .
O43 Mo39 O28 95.8(5) . .
O42 Mo39 O28 151.1(5) . .
O45 Mo39 O28 90.3(4) . .
O37 Mo39 O28 68.1(4) . .
O43 Mo39 O44 171.1(5) . .
O42 Mo39 O44 79.5(5) . .
O45 Mo39 O44 84.8(4) . .
O37 Mo39 O44 76.9(4) . .
O28 Mo39 O44 77.5(4) . .
O87 Mo40 O84 104.2(6) . .
O87 Mo40 O64 100.8(5) . .
O84 Mo40 O64 106.4(5) . .
O87 Mo40 O88 97.2(5) . .
O84 Mo40 O88 89.1(5) . .
O64 Mo40 O88 152.4(5) . .
O87 Mo40 O89 93.8(5) . .
O84 Mo40 O89 153.3(5) . .
O64 Mo40 O89 89.0(5) . .
O88 Mo40 O89 68.9(4) . .
O87 Mo40 O86 173.6(5) . .
O84 Mo40 O86 82.2(6) . .
O64 Mo40 O86 77.2(4) . .
O88 Mo40 O86 82.6(4) . .
O89 Mo40 O86 80.1(4) . .
O16 Mo41 O13 104.2(5) . .
O16 Mo41 O14 103.6(5) . .
O13 Mo41 O14 98.6(4) . .
O16 Mo41 O20 104.5(5) . .
O13 Mo41 O20 88.7(4) . .
O14 Mo41 O20 148.1(4) . .
O16 Mo41 O26 96.0(5) . .
O13 Mo41 O26 154.5(4) . .
O14 Mo41 O26 91.4(4) . .
O20 Mo41 O26 71.1(4) . .
O16 Mo41 O18 169.4(5) . .
O13 Mo41 O18 86.2(4) . .
O14 Mo41 O18 72.4(4) . .
O20 Mo41 O18 77.3(4) . .
O26 Mo41 O18 74.6(4) . .
O115 Mo42 O125 103.8(5) . 2_755
O115 Mo42 O112 99.0(5) . .
O125 Mo42 O112 90.5(4) 2_755 .
O115 Mo42 O116 101.8(5) . 2_755
O125 Mo42 O116 87.0(5) 2_755 2_755
O112 Mo42 O116 159.0(4) . 2_755
O115 Mo42 O114 99.0(5) . .
O125 Mo42 O114 157.0(4) 2_755 .
O112 Mo42 O114 88.5(4) . .
O116 Mo42 O114 85.7(4) 2_755 .
O115 Mo42 O111 166.2(5) . .
O125 Mo42 O111 88.1(4) 2_755 .
O112 Mo42 O111 73.5(4) . .
O116 Mo42 O111 85.6(4) 2_755 .
O114 Mo42 O111 69.6(4) . .
O173 Mo43 O172 100.0(5) . .
O173 Mo43 O167 95.0(5) . .
O172 Mo43 O167 141.3(4) . .
O173 Mo43 O174 95.7(5) . .
O172 Mo43 O174 71.9(4) . .
O167 Mo43 O174 141.8(4) . .
O173 Mo43 O168 100.4(5) . .
O172 Mo43 O168 71.2(4) . .
O167 Mo43 O168 71.1(4) . .
O174 Mo43 O168 141.7(4) . .
O173 Mo43 O176 94.3(5) . .
O172 Mo43 O176 141.5(4) . .
O167 Mo43 O176 71.4(4) . .
O174 Mo43 O176 71.3(4) . .
O168 Mo43 O176 140.6(4) . .
O173 Mo43 O175 167.9(5) . .
O172 Mo43 O175 89.9(4) . .
O167 Mo43 O175 81.2(4) . .
O174 Mo43 O175 80.7(4) . .
O168 Mo43 O175 89.3(4) . .
O176 Mo43 O175 73.6(4) . .
O12 Mo44 O11 98.9(5) . .
O12 Mo44 O13 104.2(5) . .
O11 Mo44 O13 89.5(4) . .
O12 Mo44 O15 101.1(5) . .
O11 Mo44 O15 160.0(4) . .
O13 Mo44 O15 86.6(4) . .
O12 Mo44 O205 99.8(5) . .
O11 Mo44 O205 89.1(4) . .
O13 Mo44 O205 155.8(4) . .
O15 Mo44 O205 86.5(4) . .
O12 Mo44 O215 167.7(5) . .
O11 Mo44 O215 74.2(4) . .
O13 Mo44 O215 86.1(4) . .
O15 Mo44 O215 86.0(4) . .
O205 Mo44 O215 70.3(4) . .
O212 Mo45 O211 100.5(5) . .
O212 Mo45 O209 100.5(5) . .
O211 Mo45 O209 70.6(4) . .
O212 Mo45 O8 94.2(5) . .
O211 Mo45 O8 73.1(4) . .
O209 Mo45 O8 142.7(4) . .
O212 Mo45 O213 94.4(5) . .
O211 Mo45 O213 141.9(5) . .
O209 Mo45 O213 72.3(4) . .
O8 Mo45 O213 140.8(4) . .
O212 Mo45 O216 96.6(5) . .
O211 Mo45 O216 140.9(4) . .
O209 Mo45 O216 139.7(4) . .
O8 Mo45 O216 70.8(4) . .
O213 Mo45 O216 70.2(4) . .
O212 Mo45 O214 170.3(5) . .
O211 Mo45 O214 87.6(4) . .
O209 Mo45 O214 87.1(4) . .
O8 Mo45 O214 83.1(4) . .
O213 Mo45 O214 82.1(4) . .
O216 Mo45 O214 73.8(4) . .
O192 Mo46 O188 104.1(6) . .
O192 Mo46 O190 100.3(5) . .
O188 Mo46 O190 105.3(5) . .
O192 Mo46 O172 95.3(5) . .
O188 Mo46 O172 90.4(5) . .
O190 Mo46 O172 154.2(5) . .
O192 Mo46 O174 96.6(5) . .
O188 Mo46 O174 151.3(5) . .
O190 Mo46 O174 90.0(4) . .
O172 Mo46 O174 67.8(4) . .
O192 Mo46 O189 172.3(5) . .
O188 Mo46 O189 82.6(5) . .
O190 Mo46 O189 81.3(5) . .
O172 Mo46 O189 80.6(4) . .
O174 Mo46 O189 75.8(4) . .
O6 Mo47 O4 103.8(7) . .
O6 Mo47 O7 100.8(5) . .
O4 Mo47 O7 106.6(5) . .
O6 Mo47 O211 96.3(5) . .
O4 Mo47 O211 89.6(5) . .
O7 Mo47 O211 152.7(5) . .
O6 Mo47 O8 95.2(5) . .
O4 Mo47 O8 152.7(5) . .
O7 Mo47 O8 88.6(4) . .
O211 Mo47 O8 68.7(4) . .
O6 Mo47 O5 172.5(5) . .
O4 Mo47 O5 83.0(6) . .
O7 Mo47 O5 80.0(5) . .
O211 Mo47 O5 80.3(4) . .
O8 Mo47 O5 77.3(4) . .
O98 Mo48 O99 104.5(7) . .
O98 Mo48 O100 100.7(6) . .
O99 Mo48 O100 99.5(6) . .
O98 Mo48 O78 91.9(6) . .
O99 Mo48 O78 96.6(7) . .
O100 Mo48 O78 156.3(5) . .
O98 Mo48 O96 164.9(6) . .
O99 Mo48 O96 89.5(6) . .
O100 Mo48 O96 82.3(4) . .
O78 Mo48 O96 80.5(4) . .
O98 Mo48 O97 91.4(6) . .
O99 Mo48 O97 162.4(6) . .
O100 Mo48 O97 84.4(5) . .
O78 Mo48 O97 75.2(5) . .
O96 Mo48 O97 74.0(4) . .
O60 Mo49 O59 99.2(8) . .
O60 Mo49 O3 102.7(6) . .
O59 Mo49 O3 97.1(7) . .
O60 Mo49 O76 93.2(6) . .
O59 Mo49 O76 90.1(8) . .
O3 Mo49 O76 161.1(5) . .
O60 Mo49 O58 92.0(7) . .
O59 Mo49 O58 166.8(6) . .
O3 Mo49 O58 87.1(5) . .
O76 Mo49 O58 82.3(6) . .
O60 Mo49 O57 170.2(7) . .
O59 Mo49 O57 88.7(6) . .
O3 Mo49 O57 81.9(4) . .
O76 Mo49 O57 80.9(5) . .
O58 Mo49 O57 79.5(5) . .
O162 Mo50 O160 105.2(7) . .
O162 Mo50 O164 102.9(6) . .
O160 Mo50 O164 104.1(6) . .
O162 Mo50 O137 95.7(5) . .
O160 Mo50 O137 91.6(5) . .
O164 Mo50 O137 151.3(5) . .
O162 Mo50 O156 94.4(5) . .
O160 Mo50 O156 153.6(5) . .
O164 Mo50 O156 88.1(4) . .
O137 Mo50 O156 68.7(4) . .
O162 Mo50 O161 171.2(5) . .
O160 Mo50 O161 80.7(6) . .
O164 Mo50 O161 81.5(5) . .
O137 Mo50 O161 77.5(4) . .
O156 Mo50 O161 78.0(4) . .
O31 Mo51 O29 103.6(5) . .
O31 Mo51 O30 107.1(5) . .
O29 Mo51 O30 100.2(4) . .
O31 Mo51 O18 104.0(5) . .
O29 Mo51 O18 96.3(4) . .
O30 Mo51 O18 139.9(4) . .
O31 Mo51 O19 98.8(5) . .
O29 Mo51 O19 157.1(4) . .
O30 Mo51 O19 77.4(4) . .
O18 Mo51 O19 73.5(4) . .
O31 Mo51 O26 176.2(5) . .
O29 Mo51 O26 73.2(4) . .
O30 Mo51 O26 75.7(4) . .
O18 Mo51 O26 74.6(4) . .
O19 Mo51 O26 84.3(3) . .
O195 Mo52 O197 105.3(6) . .
O195 Mo52 O208 102.2(5) . .
O197 Mo52 O208 103.9(5) . .
O195 Mo52 O209 93.0(5) . .
O197 Mo52 O209 92.1(5) . .
O208 Mo52 O209 154.0(5) . .
O195 Mo52 O213 94.7(5) . .
O197 Mo52 O213 153.4(5) . .
O208 Mo52 O213 88.5(4) . .
O209 Mo52 O213 69.1(4) . .
O195 Mo52 O210 171.6(5) . .
O197 Mo52 O210 80.8(6) . .
O208 Mo52 O210 81.7(5) . .
O209 Mo52 O210 80.8(5) . .
O213 Mo52 O210 77.8(4) . .
O74 Mo53 O78 100.6(7) . .
O74 Mo53 O76 103.2(8) . .
O78 Mo53 O76 104.8(6) . .
O74 Mo53 O73 97.7(6) . .
O78 Mo53 O73 154.6(5) . .
O76 Mo53 O73 87.8(5) . .
O74 Mo53 O75 99.8(6) . .
O78 Mo53 O75 90.9(5) . .
O76 Mo53 O75 149.0(6) . .
O73 Mo53 O75 68.7(4) . .
O74 Mo53 O77 175.2(6) . .
O78 Mo53 O77 77.9(6) . .
O76 Mo53 O77 81.6(7) . .
O73 Mo53 O77 82.3(5) . .
O75 Mo53 O77 75.7(4) . .
O186 Mo54 O184 104.4(8) . .
O186 Mo54 O185 98.5(6) . .
O184 Mo54 O185 99.6(6) . .
O186 Mo54 O39 94.9(6) . .
O184 Mo54 O39 92.5(5) . .
O185 Mo54 O39 159.0(5) . .
O186 Mo54 O22 91.6(7) . .
O184 Mo54 O22 163.1(6) . .
O185 Mo54 O22 83.0(5) . .
O39 Mo54 O22 80.5(4) . .
O186 Mo54 O187 165.1(7) . .
O184 Mo54 O187 89.4(6) . .
O185 Mo54 O187 84.2(5) . .
O39 Mo54 O187 78.8(5) . .
O22 Mo54 O187 74.2(5) . .
O121 Mo55 O120 103.4(7) . .
O121 Mo55 O100 97.4(7) . .
O120 Mo55 O100 98.0(5) . .
O121 Mo55 O122 98.3(9) . 2_755
O120 Mo55 O122 95.8(6) . 2_755
O100 Mo55 O122 156.1(6) . 2_755
O121 Mo55 O119 164.9(7) . .
O120 Mo55 O119 91.4(7) . .
O100 Mo55 O119 83.0(5) . .
O122 Mo55 O119 77.2(7) 2_755 .
O121 Mo55 O118 90.1(7) . .
O120 Mo55 O118 166.4(7) . .
O100 Mo55 O118 80.7(5) . .
O122 Mo55 O118 81.3(5) 2_755 .
O119 Mo55 O118 75.0(7) . .
O182 Mo56 O181 103.4(8) . .
O182 Mo56 O185 99.1(7) . .
O181 Mo56 O185 97.3(6) . .
O182 Mo56 O171 98.0(7) . .
O181 Mo56 O171 95.1(6) . .
O185 Mo56 O171 155.8(5) . .
O182 Mo56 O188 90.1(7) . .
O181 Mo56 O188 166.4(7) . .
O185 Mo56 O188 81.6(4) . .
O171 Mo56 O188 81.5(5) . .
O182 Mo56 O183 163.8(7) . .
O181 Mo56 O183 92.3(7) . .
O185 Mo56 O183 82.4(5) . .
O171 Mo56 O183 76.5(6) . .
O188 Mo56 O183 74.2(5) . .
O105 Mo57 O104 101.6(6) . .
O105 Mo57 O85 105.5(5) . .
O104 Mo57 O85 99.1(6) . .
O105 Mo57 O106 93.6(5) . .
O104 Mo57 O106 93.3(6) . .
O85 Mo57 O106 154.5(5) . .
O105 Mo57 O88 157.3(5) . .
O104 Mo57 O88 92.7(5) . .
O85 Mo57 O88 89.3(5) . .
O106 Mo57 O88 67.8(4) . .
O105 Mo57 O107 86.0(5) . .
O104 Mo57 O107 171.3(5) . .
O85 Mo57 O107 82.7(5) . .
O106 Mo57 O107 81.9(4) . .
O88 Mo57 O107 78.8(4) . .
O47 Mo58 O48 104.0(7) . .
O47 Mo58 O49 100.1(6) . .
O48 Mo58 O49 100.1(6) . .
O47 Mo58 O41 93.5(5) . .
O48 Mo58 O41 92.5(6) . .
O49 Mo58 O41 158.6(5) . .
O47 Mo58 O46 94.1(6) . .
O48 Mo58 O46 160.8(6) . .
O49 Mo58 O46 82.7(6) . .
O41 Mo58 O46 79.8(5) . .
O47 Mo58 O42 166.7(6) . .
O48 Mo58 O42 87.8(6) . .
O49 Mo58 O42 83.6(5) . .
O41 Mo58 O42 79.6(5) . .
O46 Mo58 O42 73.6(5) . .
O81 Mo59 O82 103.0(8) . .
O81 Mo59 O49 98.6(6) . .
O82 Mo59 O49 98.0(6) . .
O81 Mo59 O85 98.4(6) . .
O82 Mo59 O85 94.6(6) . .
O49 Mo59 O85 155.9(6) . .
O81 Mo59 O84 88.9(7) . .
O82 Mo59 O84 167.9(7) . .
O49 Mo59 O84 82.1(5) . .
O85 Mo59 O84 81.3(5) . .
O81 Mo59 O83 164.8(7) . .
O82 Mo59 O83 92.2(7) . .
O49 Mo59 O83 78.3(5) . .
O85 Mo59 O83 80.8(5) . .
O84 Mo59 O83 76.0(5) . .
O117 Mo60 O118 105.0(8) . 2_755
O117 Mo60 O116 99.5(6) . .
O118 Mo60 O116 106.9(6) 2_755 .
O117 Mo60 O134 95.7(6) . .
O118 Mo60 O134 88.9(5) 2_755 .
O116 Mo60 O134 154.2(5) . .
O117 Mo60 O124 94.4(6) . .
O118 Mo60 O124 151.8(6) 2_755 .
O116 Mo60 O124 89.4(5) . .
O134 Mo60 O124 68.7(4) . .
O117 Mo60 O123 170.1(6) . .
O118 Mo60 O123 83.9(7) 2_755 .
O116 Mo60 O123 81.6(5) . .
O134 Mo60 O123 80.0(5) . .
O124 Mo60 O123 75.7(5) . .
O2 Mo61 O228 102.3(10) . .
O2 Mo61 O3 98.7(6) . .
O228 Mo61 O3 97.7(8) . .
O2 Mo61 O199 95.8(7) . .
O228 Mo61 O199 96.6(10) . .
O3 Mo61 O199 156.9(8) . .
O2 Mo61 O4 167.7(9) . .
O228 Mo61 O4 89.8(8) . .
O3 Mo61 O4 81.2(5) . .
O199 Mo61 O4 80.8(6) . .
O2 Mo61 O1 88.7(9) . .
O228 Mo61 O1 168.9(8) . .
O3 Mo61 O1 80.5(6) . .
O199 Mo61 O1 81.9(9) . .
O4 Mo61 O1 79.1(6) . .
O136 Mo62 O122 106.0(6) . .
O136 Mo62 O139 94.7(7) . .
O122 Mo62 O139 94.7(8) . .
O136 Mo62 O137 94.1(5) . .
O122 Mo62 O137 158.8(6) . .
O139 Mo62 O137 90.2(6) . .
O136 Mo62 O135 91.2(6) . .
O122 Mo62 O135 89.9(7) . .
O139 Mo62 O135 171.2(6) . .
O137 Mo62 O135 82.9(5) . .
O136 Mo62 O134 162.1(5) . .
O122 Mo62 O134 91.5(6) . .
O139 Mo62 O134 87.1(5) . .
O137 Mo62 O134 68.1(4) . .
O135 Mo62 O134 85.3(5) . .
O145 Mo63 O170 103.9(7) . .
O145 Mo63 O171 103.8(6) . .
O170 Mo63 O171 100.8(7) . .
O145 Mo63 O168 93.3(5) . .
O170 Mo63 O168 95.0(6) . .
O171 Mo63 O168 153.0(6) . .
O145 Mo63 O172 154.7(5) . .
O170 Mo63 O172 94.4(6) . .
O171 Mo63 O172 89.4(5) . .
O168 Mo63 O172 67.6(4) . .
O145 Mo63 O169 81.7(6) . .
O170 Mo63 O169 172.8(7) . .
O171 Mo63 O169 81.9(7) . .
O168 Mo63 O169 80.1(5) . .
O172 Mo63 O169 78.9(5) . .
O198 Mo64 O199 109.6(6) . .
O198 Mo64 O196 96.0(8) . .
O199 Mo64 O196 95.5(10) . .
O198 Mo64 O209 93.8(5) . .
O199 Mo64 O209 154.4(7) . .
O196 Mo64 O209 92.0(7) . .
O198 Mo64 O200 90.6(7) . .
O199 Mo64 O200 85.6(10) . .
O196 Mo64 O200 172.5(7) . .
O209 Mo64 O200 84.0(7) . .
O198 Mo64 O211 161.2(5) . .
O199 Mo64 O211 88.7(6) . .
O196 Mo64 O211 86.7(6) . .
O209 Mo64 O211 67.4(4) . .
O200 Mo64 O211 85.9(6) . .
O128 Ce1 O146 70.2(4) 2_755 .
O128 Ce1 O143 131.7(5) 2_755 .
O146 Ce1 O143 132.1(5) . .
O128 Ce1 O142 72.8(4) 2_755 .
O146 Ce1 O142 73.7(4) . .
O143 Ce1 O142 145.9(5) . .
O128 Ce1 O141 103.1(6) 2_755 .
O146 Ce1 O141 145.4(5) . .
O143 Ce1 O141 78.5(6) . .
O142 Ce1 O141 72.0(6) . .
O128 Ce1 O221 144.2(5) 2_755 .
O146 Ce1 O221 97.9(6) . .
O143 Ce1 O221 81.8(6) . .
O142 Ce1 O221 71.4(6) . .
O141 Ce1 O221 67.3(7) . .
O128 Ce1 O145 130.6(4) 2_755 .
O146 Ce1 O145 66.2(4) . .
O143 Ce1 O145 70.6(5) . .
O142 Ce1 O145 114.2(5) . .
O141 Ce1 O145 126.0(6) . .
O221 Ce1 O145 65.4(5) . .
O128 Ce1 O144 74.3(4) 2_755 .
O146 Ce1 O144 72.9(4) . .
O143 Ce1 O144 74.9(6) . .
O142 Ce1 O144 139.2(5) . .
O141 Ce1 O144 139.6(5) . .
O221 Ce1 O144 136.0(6) . .
O145 Ce1 O144 71.7(5) . .
O128 Ce1 O105 65.6(4) 2_755 2_755
O146 Ce1 O105 131.3(4) . 2_755
O143 Ce1 O105 71.6(4) . 2_755
O142 Ce1 O105 110.2(5) . 2_755
O141 Ce1 O105 66.5(5) . 2_755
O221 Ce1 O105 130.1(6) . 2_755
O145 Ce1 O105 135.6(4) . 2_755
O144 Ce1 O105 76.5(4) . 2_755
O223 Ce2 O224 65.5(12) . .
O223 Ce2 O197 144.8(7) . .
O224 Ce2 O197 80.8(9) . .
O223 Ce2 O160 125.7(13) . .
O224 Ce2 O160 128.5(9) . .
O197 Ce2 O160 68.0(4) . .
O223 Ce2 O158 70.5(10) . .
O224 Ce2 O158 104.6(10) . .
O197 Ce2 O158 131.4(6) . .
O160 Ce2 O158 126.8(7) . .
O223 Ce2 O136 76.5(11) . .
O224 Ce2 O136 140.5(9) . .
O197 Ce2 O136 132.5(4) . .
O160 Ce2 O136 66.5(4) . .
O158 Ce2 O136 71.1(5) . .
O223 Ce2 O198 104.8(13) . .
O224 Ce2 O198 65.0(9) . .
O197 Ce2 O198 67.4(4) . .
O160 Ce2 O198 129.2(4) . .
O158 Ce2 O198 71.6(5) . .
O136 Ce2 O198 139.7(5) . .
O223 Ce2 O222 71.1(12) . .
O224 Ce2 O222 73.7(11) . .
O197 Ce2 O222 90.3(8) . .
O160 Ce2 O222 66.9(8) . .
O158 Ce2 O222 138.1(9) . .
O136 Ce2 O222 84.2(8) . .
O198 Ce2 O222 135.2(8) . .
O223 Ce2 O159 140.6(7) . .
O224 Ce2 O159 139.0(9) . .
O197 Ce2 O159 72.9(5) . .
O160 Ce2 O159 68.9(5) . .
O158 Ce2 O159 72.7(7) . .
O136 Ce2 O159 78.8(5) . .
O198 Ce2 O159 75.9(5) . .
O222 Ce2 O159 135.8(8) . .
O344 Na1 O221 72.2(17) . .
O344 Na1 O315 114(2) . .
O221 Na1 O315 88.7(16) . .
O344 Na1 O363 49.8(17) . .
O315 Na1 O363 138(2) . .
O344 Na1 O356 145(3) . .
O221 Na1 O356 72.9(18) . .
O315 Na1 O356 66.5(17) . .
O363 Na1 O356 152(2) . .
O344 Na1 O359 134(2) . .
O221 Na1 O359 97.4(19) . .
O315 Na1 O359 111(2) . .
O363 Na1 O359 101(2) . .
O356 Na1 O359 51.1(17) . .
O355 Na2 O337 148(2) . .
O355 Na2 O79 79.2(17) . .
O337 Na2 O79 119.2(16) . .
O355 Na2 O165 74.8(16) . 3_656
O337 Na2 O165 88.5(14) . 3_656
O79 Na2 O165 65.6(8) . 3_656
O355 Na2 O95 83.8(17) . .
O337 Na2 O95 114.5(15) . .
O79 Na2 O95 102.0(11) . .
O165 Na2 O95 156.8(13) 3_656 .
Mo49 O3 Mo61 132.8(7) . .
Mo47 O4 Mo61 148.1(8) . .
Mo47 O7 Mo1 149.7(6) . .
Mo18 O8 Mo45 109.8(5) . .
Mo18 O8 Mo47 143.5(5) . .
Mo45 O8 Mo47 106.4(5) . .
Mo18 O10 Mo1 157.7(6) . .
Mo18 O11 Mo44 124.7(5) . .
Mo41 O13 Mo44 158.2(6) . .
Mo41 O14 Mo1 123.9(5) . .
Mo37 O15 Mo44 148.9(6) . .
Mo51 O18 Mo1 103.1(4) . .
Mo51 O18 Mo41 106.8(4) . .
Mo1 O18 Mo41 88.4(3) . .
Mo1 O19 Mo2 137.4(6) . .
Mo1 O19 Mo51 113.7(5) . .
Mo2 O19 Mo51 106.6(5) . .
Mo38 O20 Mo41 109.8(5) . .
Mo38 O20 Mo37 109.1(5) . .
Mo41 O20 Mo37 141.0(5) . .
Mo37 O22 Mo54 155.0(7) . .
Mo38 O25 Mo35 109.6(5) . .
Mo38 O25 Mo37 110.5(5) . .
Mo35 O25 Mo37 133.9(5) . .
Mo3 O26 Mo41 142.0(5) . .
Mo3 O26 Mo38 102.6(4) . .
Mo41 O26 Mo38 103.0(4) . .
Mo3 O26 Mo51 101.2(4) . .
Mo41 O26 Mo51 104.1(4) . .
Mo38 O26 Mo51 95.0(4) . .
Mo3 O28 Mo38 107.8(5) . .
Mo3 O28 Mo39 142.2(5) . .
Mo38 O28 Mo39 109.3(4) . .
Mo51 O29 Mo38 117.0(5) . .
Mo51 O30 Mo2 103.3(4) . .
Mo51 O30 Mo3 108.5(4) . .
Mo2 O30 Mo3 89.2(3) . .
Mo3 O32 Mo2 120.6(5) . .
Mo28 O34 Mo2 148.9(6) . .
Mo5 O35 Mo2 158.2(6) . .
Mo3 O36 Mo4 158.5(6) . .
Mo38 O37 Mo35 109.2(5) . .
Mo38 O37 Mo39 111.3(5) . .
Mo35 O37 Mo39 138.8(6) . .
Mo35 O39 Mo54 157.1(6) . .
Mo35 O41 Mo58 156.8(7) . .
Mo39 O42 Mo58 155.4(7) . .
Mo39 O45 Mo4 146.6(6) . .
C1 O46 Mo58 142.4(16) . .
Mo58 O49 Mo59 140.2(7) . .
Mo32 O50 Mo4 103.2(4) . .
Mo32 O50 Mo5 105.6(4) . .
Mo4 O50 Mo5 89.1(4) . .
Mo5 O51 Mo4 122.7(5) . .
Mo5 O53 Mo27 108.7(5) . .
Mo5 O53 Mo28 141.8(5) . .
Mo27 O53 Mo28 108.1(5) . .
Mo28 O57 Mo49 157.0(7) . .
Mo4 O61 Mo7 139.3(6) . .
Mo4 O61 Mo32 111.7(5) . .
Mo7 O61 Mo32 107.0(5) . .
Mo19 O63 Mo7 158.2(6) . .
Mo40 O64 Mo7 149.0(7) . .
Mo6 O65 Mo7 122.1(5) . .
Mo32 O66 Mo7 102.9(5) . .
Mo32 O66 Mo6 108.9(4) . .
Mo7 O66 Mo6 89.5(4) . .
Mo5 O68 Mo6 141.6(5) . .
Mo5 O68 Mo27 103.4(4) . .
Mo6 O68 Mo27 103.1(4) . .
Mo5 O68 Mo32 104.5(4) . .
Mo6 O68 Mo32 99.9(4) . .
Mo27 O68 Mo32 95.7(4) . .
Mo32 O69 Mo27 116.8(5) . .
Mo6 O70 Mo27 109.3(5) . .
Mo6 O70 Mo21 141.9(5) . .
Mo27 O70 Mo21 108.4(5) . .
Mo27 O73 Mo53 109.9(5) . .
Mo27 O73 Mo28 110.6(5) . .
Mo53 O73 Mo28 136.7(5) . .
Mo27 O75 Mo53 109.5(5) . .
Mo27 O75 Mo21 110.5(4) . .
Mo53 O75 Mo21 139.7(5) . .
Mo53 O76 Mo49 143.8(10) . .
Mo53 O78 Mo48 157.1(7) . .
Mo21 O79 Na2 117.2(8) . .
Mo40 O84 Mo59 147.4(7) . .
Mo57 O85 Mo59 159.5(7) . .
Mo33 O88 Mo40 111.5(5) . .
Mo33 O88 Mo57 108.1(5) . .
Mo40 O88 Mo57 138.3(6) . .
Mo19 O89 Mo33 109.1(5) . .
Mo19 O89 Mo40 142.9(6) . .
Mo33 O89 Mo40 106.9(5) . .
Mo36 O91 Mo8 103.0(4) . .
Mo36 O91 Mo19 107.7(4) . .
Mo8 O91 Mo19 88.6(3) . .
Mo19 O92 Mo8 123.2(5) . .
Mo21 O93 Mo8 148.2(6) . .
Mo6 O94 Mo8 158.6(6) . .
Mo8 O95 Na2 108.3(8) . .
Mo21 O96 Mo48 152.1(6) . .
C12 O97 Mo48 130.1(16) . .
Mo48 O100 Mo55 135.4(7) . .
Mo19 O101 Mo22 140.7(5) . .
Mo19 O101 Mo33 102.6(4) . .
Mo22 O101 Mo33 103.5(4) . .
Mo19 O101 Mo36 104.1(4) . .
Mo22 O101 Mo36 101.5(4) . .
Mo33 O101 Mo36 96.3(4) . .
Mo36 O102 Mo33 118.2(5) . .
Mo57 O105 Ce1 154.1(7) . 2_755
Mo33 O106 Mo57 112.1(5) . .
Mo33 O106 Mo26 110.6(5) . .
Mo57 O106 Mo26 132.7(6) . .
Mo22 O108 Mo33 110.9(5) . .
Mo22 O108 Mo26 140.9(5) . .
Mo33 O108 Mo26 106.7(5) . .
Mo22 O110 Mo11 156.4(6) 2_755 .
Mo36 O111 Mo42 103.1(4) . .
Mo36 O111 Mo22 107.4(4) . .
Mo42 O111 Mo22 88.9(4) . .
Mo22 O112 Mo42 124.9(5) . .
Mo8 O114 Mo42 136.3(5) . .
Mo8 O114 Mo36 112.8(5) . .
Mo42 O114 Mo36 109.0(4) . .
Mo60 O116 Mo42 151.0(6) . 2_755
M60 O118 Mo55 149.1(10) . .
Mo60 O118 Mo55 154.6(8) 2_755 .
C12 O119 Mo55 128.4(12) . .
Mo62 O122 Mo55 156.2(10) . 2_755
Mo9 O124 Mo25 110.7(5) . .
Mo9 O124 Mo60 142.7(6) . .
Mo25 O124 Mo60 106.5(5) . .
Mo9 O125 Mo42 155.1(6) . 2_755
Mo26 O128 Ce1 161.5(6) . 2_755
Mo26 O129 Mo11 151.8(6) 2_755 .
Mo9 O131 Mo11 123.3(5) . .
Mo10 O132 Mo11 102.6(4) . .
Mo10 O132 Mo9 106.0(4) . .
Mo11 O132 Mo9 89.2(3) . .
Mo25 O134 Mo60 110.6(5) . .
Mo25 O134 Mo62 109.4(5) . .
Mo60 O134 Mo62 132.2(6) . .
Mo62 O136 Ce2 161.4(7) . .
Mo25 O137 Mo62 111.5(5) . .
Mo25 O137 Mo50 110.5(5) . .
Mo62 O137 Mo50 133.8(5) . .
Mo10 O140 Mo25 116.9(5) . .
Mo63 O145 Ce1 161.4(7) . .
Mo30 O146 Ce1 151.1(6) . .
Mo30 O149 Mo23 150.9(6) . .
Mo11 O152 Mo23 138.0(5) . .
Mo11 O152 Mo10 112.6(5) . .
Mo23 O152 Mo10 109.3(5) . .
Mo10 O153 Mo20 107.6(4) . .
Mo10 O153 Mo23 103.8(4) . .
Mo20 O153 Mo23 90.5(3) . .
Mo20 O154 Mo23 120.9(5) . .
Mo9 O155 Mo20 146.4(5) . .
Mo9 O155 Mo25 101.9(4) . .
Mo20 O155 Mo25 101.9(4) . .
Mo9 O155 Mo10 102.7(4) . .
Mo20 O155 Mo10 98.0(4) . .
Mo25 O155 Mo10 96.1(4) . .
Mo20 O156 Mo25 110.9(5) . .
Mo20 O156 Mo50 140.6(5) . .
Mo25 O156 Mo50 106.8(4) . .
Mo50 O160 Ce2 164.3(8) . .
Mo20 O163 Mo29 153.1(6) . .
Mo50 O164 Mo29 150.0(6) . .
Mo29 O165 Na2 134.7(9) . 3_646
Mo24 O166 Mo29 103.0(4) . .
Mo24 O166 Mo12 105.8(4) . .
Mo29 O166 Mo12 89.2(3) . .
Mo43 O167 Mo12 110.0(5) . .
Mo43 O167 Mo30 108.6(5) . .
Mo12 O167 Mo30 141.2(5) . .
Mo43 O168 Mo63 111.5(5) . .
Mo43 O168 Mo30 111.2(5) . .
Mo63 O168 Mo30 135.7(6) . .
Mo63 O171 Mo56 148.2(9) . .
Mo43 O172 Mo46 111.3(5) . .
Mo43 O172 Mo63 109.2(5) . .
Mo46 O172 Mo63 137.0(6) . .
Mo13 O174 Mo43 110.3(5) . .
Mo13 O174 Mo46 142.0(5) . .
Mo43 O174 Mo46 107.6(5) . .
Mo24 O175 Mo43 116.2(5) . .
Mo12 O176 Mo13 146.8(5) . .
Mo12 O176 Mo43 101.8(4) . .
Mo13 O176 Mo43 101.5(4) . .
Mo12 O176 Mo24 102.9(4) . .
Mo13 O176 Mo24 98.0(4) . .
Mo43 O176 Mo24 95.6(4) . .
Mo12 O178 Mo29 123.3(5) . .
C23 O183 Mo56 130.0(12) . .
Mo54 O185 Mo56 135.5(7) . .
C23 O187 Mo54 128.4(12) . .
Mo46 O188 Mo56 152.1(6) . .
Mo46 O190 Mo15 150.8(7) . .
Mo29 O193 Mo14 136.4(5) . .
Mo29 O193 Mo24 114.4(5) . .
Mo14 O193 Mo24 109.1(5) . .
Mo24 O194 Mo14 104.1(4) . .
Mo24 O194 Mo13 108.0(4) . .
Mo14 O194 Mo13 89.3(3) . .
Mo52 O197 Ce2 153.9(8) . .
Mo64 O198 Ce2 162.2(7) . .
Mo64 O199 Mo61 156.5(12) . .
Mo13 O203 Mo14 122.5(5) . .
Mo13 O204 Mo15 155.6(7) . .
Mo15 O205 Mo44 135.8(6) . .
Mo15 O205 Mo34 114.0(5) . .
Mo44 O205 Mo34 108.0(5) . .
Mo31 O206 Mo15 125.8(5) . .
Mo52 O208 Mo14 150.7(6) . .
Mo45 O209 Mo64 112.0(5) . .
Mo45 O209 Mo52 110.4(5) . .
Mo64 O209 Mo52 133.5(6) . .
Mo45 O211 Mo47 110.9(5) . .
Mo45 O211 Mo64 109.9(5) . .
Mo47 O211 Mo64 135.1(6) . .
Mo31 O213 Mo45 109.4(5) . .
Mo31 O213 Mo52 142.9(5) . .
Mo45 O213 Mo52 107.2(5) . .
Mo34 O214 Mo45 118.2(5) . .
Mo34 O215 Mo44 103.5(4) . .
Mo34 O215 Mo18 107.3(5) . .
Mo44 O215 Mo18 88.0(3) . .
Mo31 O216 Mo18 142.3(6) . .
Mo31 O216 Mo45 103.7(4) . .
Mo18 O216 Mo45 102.3(4) . .
Mo34 O217 Mo15 103.4(4) . .
Mo34 O217 Mo31 106.2(4) . .
Mo15 O217 Mo31 87.8(4) . .
Mo31 O219 Mo14 156.6(6) . .
Mo12 O220 Mo23 155.7(6) . .
Na1 O221 Ce1 144.1(14) . .
C5 N2 C6 113(2) . .
C16 N3 C18 110(2) . .
C29 N6 C27 107.9(18) . .
O46 C1 O225 125(2) . .
O46 C1 C2 117(2) . .
O225 C1 C2 118(2) . .
O225 C1 M58 99.4(16) . .
C2 C1 M58 142.5(17) . .
N1 C2 C1 107.7(18) . .
N1 C2 C3 114.2(19) . .
C1 C2 C3 108.7(19) . .
C4 C3 C2 109(2) . .
C7 C4 C5 106(2) . .
C7 C4 C3 127(2) . .
C5 C4 C3 126(2) . .
N2 C5 C4 108(3) . .
C11 C6 N2 129(3) . .
C11 C6 C7 125(3) . .
N2 C6 C7 106(2) . .
C6 C7 C8 118(3) . .
C6 C7 C4 107(2) . .
C8 C7 C4 134(2) . .
C7 C8 C9 117(3) . .
C10 C9 C8 122(4) . .
C9 C10 C11 120(4) . .
C6 C11 C10 117(3) . .
O119 C12 O97 128.5(19) . .
O119 C12 C13 124.4(19) . .
O97 C12 C13 107(2) . .
N4 C13 C14 112(3) . .
N4 C13 C12 110(2) . .
C14 C13 C12 92(2) . .
C13 C14 C15 97(3) . .
C17 C15 C16 100(2) . .
C17 C15 C14 133(3) . .
C16 C15 C14 127(3) . .
N3 C16 C15 112(2) . .
C18 C17 C15 109(3) . .
C18 C17 C22 120(3) . .
C15 C17 C22 129(3) . .
N3 C18 C17 107(3) . .
N3 C18 C19 126(4) . .
C17 C18 C19 126(4) . .
C20 C19 C18 110(6) . .
C19 C20 C21 131(7) . .
C20 C21 C22 119(5) . .
C17 C22 C21 112(4) . .
O187 C23 O183 125.3(17) . .
O187 C23 C24 118.4(16) . .
O183 C23 C24 115.9(16) . .
N5 C24 C23 111.0(16) . .
N5 C24 C25 109.3(14) . .
C23 C24 C25 110.7(15) . .
C24 C25 C26 112.6(16) . .
C27 C26 C28 109.1(17) . .
C27 C26 C25 126.9(19) . .
C28 C26 C25 124.1(17) . .
C26 C27 N6 109(2) . .
C33 C28 C26 136(2) . .
C33 C28 C29 118(3) . .
C26 C28 C29 106.2(18) . .
N6 C29 C28 107.6(19) . .
N6 C29 C30 129(2) . .
C28 C29 C30 123(3) . .
C31 C30 C29 115(3) . .
C32 C31 C30 118(3) . .
C31 C32 C33 126(4) . .
C28 C33 C32 117(3) . .
O227 C34 O226 125(3) . .
O227 C34 C35 120(3) . .
O226 C34 C35 114(3) . .
C34 C35 N8 113.9(19) . .
C34 C35 C36 112(2) . .
N8 C35 C36 111(2) . .
C37 C36 C35 111.3(18) . .
O229 C37 C40 122(2) . .
O229 C37 C36 119(2) . .
C40 C37 C36 118.8(19) . .
C44 C39 N7 117(2) . .
C44 C39 C40 123(2) . .
N7 C39 C40 120.3(19) . .
C37 C40 C39 122.4(19) . .
C37 C40 C41 121(2) . .
C39 C40 C41 116.9(19) . .
C42 C41 C40 120(2) . .
C41 C42 C43 119(2) . .
C44 C43 C42 122.7(19) . .
C39 C44 C43 118(2) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O17 1.675(10) .
Mo1 O10 1.890(10) .
Mo1 O14 1.940(10) .
Mo1 O7 1.955(11) .
Mo1 O19 1.995(11) .
Mo1 O18 2.344(10) .
Mo2 O33 1.678(11) .
Mo2 O35 1.925(10) .
Mo2 O32 1.958(10) .
Mo2 O34 1.958(10) .
Mo2 O19 2.007(10) .
Mo2 O30 2.287(10) .
Mo3 O27 1.687(10) .
Mo3 O36 1.852(11) .
Mo3 O32 1.859(10) .
Mo3 O28 2.003(10) .
Mo3 O26 2.071(10) .
Mo3 O30 2.432(9) .
Mo4 O52 1.684(10) .
Mo4 O36 1.900(11) .
Mo4 O51 1.942(10) .
Mo4 O45 1.973(11) .
Mo4 O61 1.995(11) .
Mo4 O50 2.282(10) .
Mo5 O54 1.672(10) .
Mo5 O35 1.834(11) .
Mo5 O51 1.863(9) .
Mo5 O53 1.994(10) .
Mo5 O68 2.059(10) .
Mo5 O50 2.475(10) .
Mo6 O71 1.677(10) .
Mo6 O94 1.833(11) .
Mo6 O65 1.867(10) .
Mo6 O70 1.997(10) .
Mo6 O68 2.078(10) .
Mo6 O66 2.406(10) .
Mo7 O62 1.685(11) .
Mo7 O63 1.905(11) .
Mo7 O65 1.940(10) .
Mo7 O64 1.947(11) .
Mo7 O61 2.013(11) .
Mo7 O66 2.327(11) .
Mo8 O95 1.665(11) .
Mo8 O94 1.914(11) .
Mo8 O92 1.945(11) .
Mo8 O93 1.964(10) .
Mo8 O114 2.000(10) .
Mo8 O91 2.343(10) .
Mo9 O133 1.663(10) .
Mo9 O125 1.872(10) .
Mo9 O131 1.876(10) .
Mo9 O124 1.985(10) .
Mo9 O155 2.085(11) .
Mo9 O132 2.390(10) .
Mo10 O151 1.676(10) .
Mo10 O140 1.779(10) .
Mo10 O153 1.907(10) .
Mo10 O132 2.009(10) .
Mo10 O152 2.126(10) .
Mo10 O155 2.416(10) .
Mo11 O130 1.673(11) .
Mo11 O110 1.900(10) .
Mo11 O131 1.917(10) .
Mo11 O129 1.954(10) .
Mo11 O152 1.986(10) .
Mo11 O132 2.365(10) .
Mo12 O177 1.674(10) .
Mo12 O220 1.861(10) .
Mo12 O178 1.873(10) .
Mo12 O167 1.995(10) .
Mo12 O176 2.090(10) .
Mo12 O166 2.399(10) .
Mo13 O201 1.676(11) .
Mo13 O204 1.859(10) .
Mo13 O203 1.873(10) .
Mo13 O174 1.989(11) .
Mo13 O176 2.110(10) .
Mo13 O194 2.366(10) .
Mo14 O207 1.668(12) .
Mo14 O219 1.894(10) .
Mo14 O203 1.914(10) .
Mo14 O208 1.949(10) .
Mo14 O193 2.002(11) .
Mo14 O194 2.359(10) .
Mo15 O202 1.674(11) .
Mo15 O204 1.905(11) .
Mo15 O206 1.919(10) .
Mo15 O190 1.974(11) .
Mo15 O205 2.006(10) .
Mo15 O217 2.352(11) .
Mo18 O9 1.676(10) .
Mo18 O11 1.844(10) .
Mo18 O10 1.858(10) .
Mo18 O8 1.974(11) .
Mo18 O216 2.073(10) .
Mo18 O215 2.477(10) .
Mo19 O90 1.681(11) .
Mo19 O63 1.854(11) .
Mo19 O92 1.859(11) .
Mo19 O89 1.988(10) .
Mo19 O101 2.067(10) .
Mo19 O91 2.447(10) .
Mo20 O157 1.682(10) .
Mo20 O163 1.861(10) .
Mo20 O154 1.889(9) .
Mo20 O156 1.971(9) .
Mo20 O155 2.102(10) .
Mo20 O153 2.315(10) .
Mo21 O80 1.695(10) .
Mo21 O96 1.774(10) .
Mo21 O93 1.839(11) .
Mo21 O75 2.062(10) .
Mo21 O70 2.106(10) .
Mo21 O79 2.374(11) .
Mo22 O109 1.664(10) .
Mo22 O112 1.852(10) .
Mo22 O110 1.852(11) 2_755
Mo22 O108 1.985(10) .
Mo22 O101 2.074(10) .
Mo22 O111 2.461(10) .
Mo23 O150 1.667(11) .
Mo23 O220 1.912(10) .
Mo23 O154 1.927(9) .
Mo23 O149 1.966(10) .
Mo23 O152 2.002(11) .
Mo23 O153 2.360(10) .
Mo24 O179 1.675(11) .
Mo24 O175 1.763(10) .
Mo24 O194 1.878(10) .
Mo24 O166 2.048(10) .
Mo24 O193 2.114(10) .
Mo24 O176 2.445(9) .
Mo25 O138 1.691(10) .
Mo25 O134 1.985(11) .
Mo25 O124 1.999(10) .
Mo25 O137 2.013(10) .
Mo25 O156 2.024(10) .
Mo25 O155 2.135(9) .
Mo25 O140 2.190(10) .
Mo26 O126 1.702(11) .
Mo26 O128 1.762(11) .
Mo26 O129 1.830(11) 2_755
Mo26 O106 2.065(11) .
Mo26 O108 2.142(10) .
Mo26 O127 2.353(12) .
Mo27 O72 1.691(11) .
Mo27 O73 1.984(10) .
Mo27 O75 1.991(10) .
Mo27 O70 1.999(10) .
Mo27 O53 2.006(11) .
Mo27 O68 2.084(10) .
Mo27 O69 2.185(10) .
Mo28 O55 1.688(11) .
Mo28 O57 1.773(10) .
Mo28 O34 1.850(10) .
Mo28 O73 2.060(11) .
Mo28 O53 2.101(10) .
Mo28 O56 2.350(10) .
Mo29 O165 1.671(11) .
Mo29 O163 1.910(10) .
Mo29 O178 1.919(10) .
Mo29 O164 1.948(10) .
Mo29 O193 1.991(10) .
Mo29 O166 2.355(9) .
Mo30 O148 1.704(11) .
Mo30 O146 1.743(10) .
Mo30 O149 1.827(10) .
Mo30 O168 2.044(10) .
Mo30 O167 2.118(10) .
Mo30 O147 2.328(11) .
Mo31 O218 1.683(10) .
Mo31 O219 1.860(11) .
Mo31 O206 1.862(10) .
Mo31 O213 1.981(11) .
Mo31 O216 2.049(10) .
Mo31 O217 2.499(10) .
Mo32 O67 1.680(11) .
Mo32 O69 1.804(10) .
Mo32 O66 1.894(11) .
Mo32 O50 2.045(11) .
Mo32 O61 2.107(11) .
Mo32 O68 2.493(10) .
Mo33 O103 1.681(11) .
Mo33 O106 1.989(11) .
Mo33 O88 1.991(11) .
Mo33 O108 2.011(10) .
Mo33 O89 2.018(11) .
Mo33 O101 2.114(10) .
Mo33 O102 2.215(10) .
Mo34 O191 1.664(11) .
Mo34 O214 1.769(10) .
Mo34 O215 1.896(11) .
Mo34 O217 2.035(11) .
Mo34 O205 2.107(11) .
Mo35 O40 1.684(13) .
Mo35 O41 1.785(12) .
Mo35 O39 1.791(12) .
Mo35 O37 2.043(11) .
Mo35 O25 2.050(12) .
Mo35 O38 2.452(12) .
Mo36 O113 1.670(10) .
Mo36 O102 1.778(10) .
Mo36 O111 1.912(11) .
Mo36 O91 1.998(10) .
Mo36 O114 2.088(10) .
Mo36 O101 2.483(10) .
Mo37 O21 1.688(12) .
Mo37 O22 1.760(11) .
Mo37 O15 1.828(11) .
Mo37 O25 2.072(11) .
Mo37 O20 2.094(10) .
Mo37 O23 2.341(13) .
Mo38 O24 1.694(11) .
Mo38 O25 1.980(10) .
Mo38 O20 1.993(10) .
Mo38 O37 1.996(10) .
Mo38 O28 2.012(10) .
Mo38 O26 2.087(10) .
Mo38 O29 2.204(10) .
Mo39 O43 1.712(10) .
Mo39 O42 1.751(11) .
Mo39 O45 1.836(11) .
Mo39 O37 2.058(11) .
Mo39 O28 2.091(10) .
Mo39 O44 2.361(10) .
Mo40 O87 1.691(10) .
Mo40 O84 1.731(11) .
Mo40 O64 1.860(11) .
Mo40 O88 2.029(11) .
Mo40 O89 2.118(11) .
Mo40 O86 2.342(11) .
Mo41 O16 1.662(11) .
Mo41 O13 1.825(11) .
Mo41 O14 1.859(10) .
Mo41 O20 2.000(10) .
Mo41 O26 2.086(10) .
Mo41 O18 2.463(10) .
Mo42 O115 1.687(10) .
Mo42 O125 1.903(10) 2_755
Mo42 O112 1.940(10) .
Mo42 O116 1.964(11) 2_755
Mo42 O114 2.017(11) .
Mo42 O111 2.341(10) .
Mo43 O173 1.688(11) .
Mo43 O172 1.961(11) .
Mo43 O167 1.995(10) .
Mo43 O174 2.004(10) .
Mo43 O168 2.005(11) .
Mo43 O176 2.122(10) .
Mo43 O175 2.219(10) .
Mo44 O12 1.676(11) .
Mo44 O11 1.929(10) .
Mo44 O13 1.935(11) .
Mo44 O15 1.976(11) .
Mo44 O205 2.011(10) .
Mo44 O215 2.332(11) .
Mo45 O212 1.685(11) .
Mo45 O211 1.967(11) .
Mo45 O209 1.999(11) .
Mo45 O8 2.006(10) .
Mo45 O213 2.023(10) .
Mo45 O216 2.107(10) .
Mo45 O214 2.246(10) .
Mo46 O192 1.708(12) .
Mo46 O188 1.769(10) .
Mo46 O190 1.834(11) .
Mo46 O172 2.061(10) .
Mo46 O174 2.111(11) .
Mo46 O189 2.351(12) .
Mo47 O6 1.714(12) .
Mo47 O4 1.760(11) .
Mo47 O7 1.860(10) .
Mo47 O211 2.056(11) .
Mo47 O8 2.133(11) .
Mo47 O5 2.341(13) .
Mo48 O98 1.694(13) .
Mo48 O99 1.705(14) .
Mo48 O100 1.881(12) .
Mo48 O78 2.030(13) .
Mo48 O96 2.209(10) .
Mo48 O97 2.230(12) .
Mo49 O60 1.681(13) .
Mo49 O59 1.819(17) .
Mo49 O3 1.875(12) .
Mo49 O76 2.039(14) .
Mo49 O58 2.181(15) .
Mo49 O57 2.181(11) .
Mo50 O162 1.670(12) .
Mo50 O160 1.726(11) .
Mo50 O164 1.841(11) .
Mo50 O137 2.056(11) .
Mo50 O156 2.140(10) .
Mo50 O161 2.375(11) .
Mo51 O31 1.670(11) .
Mo51 O29 1.765(10) .
Mo51 O30 1.913(10) .
Mo51 O18 2.040(10) .
Mo51 O19 2.111(10) .
Mo51 O26 2.498(9) .
Mo52 O195 1.695(12) .
Mo52 O197 1.756(12) .
Mo52 O208 1.839(10) .
Mo52 O209 2.062(10) .
Mo52 O213 2.119(11) .
Mo52 O210 2.361(12) .
Mo53 O74 1.666(14) .
Mo53 O78 1.781(12) .
Mo53 O76 1.797(13) .
Mo53 O73 2.049(10) .
Mo53 O75 2.053(10) .
Mo53 O77 2.365(15) .
Mo54 O186 1.700(14) .
Mo54 O184 1.710(12) .
Mo54 O185 1.900(12) .
Mo54 O39 2.017(12) .
Mo54 O22 2.184(11) .
Mo54 O187 2.260(13) .
Mo55 O121 1.685(15) .
Mo55 O120 1.717(12) .
Mo55 O100 1.938(12) .
Mo55 O122 1.968(15) 2_755
Mo55 O119 2.211(16) .
Mo55 O118 2.215(12) .
Mo56 O182 1.662(15) .
Mo56 O181 1.713(14) .
Mo56 O185 1.917(12) .
Mo56 O171 1.993(12) .
Mo56 O188 2.198(11) .
Mo56 O183 2.237(13) .
Mo57 O105 1.715(11) .
Mo57 O104 1.768(13) .
Mo57 O85 1.825(12) .
Mo57 O106 2.049(11) .
Mo57 O88 2.146(11) .
Mo57 O107 2.243(12) .
Mo58 O47 1.709(13) .
Mo58 O48 1.715(13) .
Mo58 O49 1.825(12) .
Mo58 O41 2.037(13) .
Mo58 O46 2.189(13) .
Mo58 O42 2.222(12) .
Mo59 O81 1.689(15) .
Mo59 O82 1.693(13) .
Mo59 O49 1.921(12) .
Mo59 O85 1.963(12) .
Mo59 O84 2.220(12) .
Mo59 O83 2.296(14) .
Mo60 O117 1.690(13) .
Mo60 O118 1.742(12) 2_755
Mo60 O116 1.831(12) .
Mo60 O134 2.043(11) .
Mo60 O124 2.135(11) .
Mo60 O123 2.304(13) .
Mo61 O2 1.714(14) .
Mo61 O228 1.72(2) .
Mo61 O3 1.904(12) .
Mo61 O199 1.955(15) .
Mo61 O4 2.176(12) .
Mo61 O1 2.229(18) .
Mo62 O136 1.725(12) .
Mo62 O122 1.772(14) .
Mo62 O139 1.940(15) .
Mo62 O137 2.033(11) .
Mo62 O135 2.076(14) .
Mo62 O134 2.112(11) .
Mo63 O145 1.726(13) .
Mo63 O170 1.751(14) .
Mo63 O171 1.821(13) .
Mo63 O168 2.027(10) .
Mo63 O172 2.125(11) .
Mo63 O169 2.344(14) .
Mo64 O198 1.709(12) .
Mo64 O199 1.761(15) .
Mo64 O196 1.923(16) .
Mo64 O209 2.026(11) .
Mo64 O200 2.091(18) .
Mo64 O211 2.107(11) .
M58 C1 2.63(3) .
M60 O118 1.73(2) .
Ce1 O128 2.452(11) 2_755
Ce1 O146 2.502(10) .
Ce1 O143 2.503(14) .
Ce1 O142 2.505(12) .
Ce1 O141 2.533(14) .
Ce1 O221 2.543(14) .
Ce1 O145 2.550(12) .
Ce1 O144 2.554(12) .
Ce1 O105 2.617(11) 2_755
Ce2 O223 2.44(2) .
Ce2 O224 2.45(4) .
Ce2 O197 2.463(12) .
Ce2 O160 2.476(11) .
Ce2 O158 2.482(18) .
Ce2 O136 2.530(12) .
Ce2 O198 2.545(12) .
Ce2 O222 2.55(3) .
Ce2 O159 2.563(13) .
Na1 O344 2.27(6) .
Na1 O221 2.52(5) .
Na1 O315 2.61(5) .
Na1 O363 2.79(7) .
Na1 O356 2.80(8) .
Na1 O359 2.81(7) .
Na2 O355 2.25(6) .
Na2 O337 2.49(5) .
Na2 O79 2.76(4) .
Na2 O165 2.86(3) 3_656
Na2 O95 2.97(3) .
O46 C1 1.21(3) .
O97 C12 1.27(3) .
O119 C12 1.25(3) .
O183 C23 1.28(2) .
O187 C23 1.25(2) .
O225 C1 1.28(3) .
O226 C34 1.32(3) .
O227 C34 1.22(3) .
O229 C37 1.23(3) .
N1 C2 1.44(3) .
N2 C5 1.30(3) .
N2 C6 1.40(3) .
N3 C16 1.30(3) .
N3 C18 1.31(3) .
N4 C13 1.49(5) .
N5 C24 1.46(2) .
N6 C29 1.37(3) .
N6 C27 1.38(3) .
N7 C39 1.43(3) .
N8 C35 1.53(3) .
C1 C2 1.56(3) .
C2 C3 1.62(3) .
C3 C4 1.52(3) .
C4 C7 1.43(4) .
C4 C5 1.45(4) .
C6 C11 1.39(4) .
C6 C7 1.41(3) .
C7 C8 1.42(4) .
C8 C9 1.45(5) .
C9 C10 1.40(5) .
C10 C11 1.43(5) .
C12 C13 1.64(4) .
C13 C14 1.53(4) .
C14 C15 1.74(5) .
C15 C17 1.41(4) .
C15 C16 1.43(4) .
C17 C18 1.40(4) .
C17 C22 1.45(5) .
C18 C19 1.41(7) .
C19 C20 1.32(8) .
C20 C21 1.35(7) .
C21 C22 1.49(6) .
C23 C24 1.53(3) .
C24 C25 1.55(3) .
C25 C26 1.56(2) .
C26 C27 1.35(3) .
C26 C28 1.38(3) .
C28 C33 1.35(4) .
C28 C29 1.42(3) .
C29 C30 1.42(4) .
C30 C31 1.41(5) .
C31 C32 1.33(4) .
C32 C33 1.40(5) .
C34 C35 1.48(4) .
C35 C36 1.54(3) .
C36 C37 1.51(3) .
C37 C40 1.43(3) .
C39 C44 1.38(3) .
C39 C40 1.45(3) .
C40 C41 1.45(3) .
C41 C42 1.39(3) .
C42 C43 1.41(3) .
C43 C44 1.40(3) .
